Talk:BPG Support Problems
Possible reorganization after split with a Support Material page
This section presents issues in the conservation treatment, storage, and/or exhibition of paper (or other) supports. These issues may relate to inherent properties of the support fibers, support manufacture, and fabrication of the object including additives, or changes in the support resulting from natural aging processes, environmental and handling conditions, or conservation treatment.
The purpose of the chapter is to outline potential problems of paper supports and related materials which may influence the course of conservation treatments, storage, and exhibition of these materials, and suggest treatment approaches.
Original Compilers: Thea Burns (Jirat-Wasiutynski) and Karen Potje
For a full list of the original contributors to this page, see the section below on History of this Chapter below.
Wiki Contributors: Jennifer Evers, Emily Williams, your name could be here
- 1 Factors to Consider
- 1.1 Inherent Physical Characteristics of Paper
- 1.2 Chemical Stability
- 1.3 Sensitivity of Paper to Its Environment
- 1.4 Alteration of Paper Support upon Aging
- 1.5 Potential Alteration of Support During Handling
- 1.6 Potential Alteration of Support During Conservation Treatment
- 1.7 Relationship of Media to Support
- 2 Treatment Variations: Support Types
- 2.1 Traditional Western Papers
- 2.1.1 Rag Papers
- 2.1.2 Mechanical Wood Pulp Papers
- 2.1.3 Chemi-Mechanical and Semi-Mechanical Pulp Papers
- 2.1.4 Chemical Wood Pulp Papers
- 2.1.5 Alum-Rosin Sized Papers
- 2.1.6 Colored Papers
- 2.1.7 Calendered Papers
- 2.1.8 Loaded Papers
- 2.1.9 Artists' Coated (Prepared) Papers
- 2.1.10 Coated Papers
- 2.1.11 Western Tissue Papers
- 2.1.12 Tracing Papers
- 2.1.13 Cardboard/Artists' Board/Illustration Board
- 2.1.14 Drawing Papers
- 2.1.15 Watercolor Papers
- 2.1.16 Artists' Printing Papers
- 2.2 Asian Papers
- 2.3 Composite Structures
- 2.4 Over-Sized/Three-Dimensional/Unusual Shapes
- 2.5 Traditional Non-Paper Supports
- 2.6 Contemporary Non-Paper Drawing Supports
- 2.1 Traditional Western Papers
- 3 Bibliography
- 3.1 General
- 3.2 Mechanical Wood Pulp Papers
- 3.3 Colored Papers
- 3.4 Loaded Papers
- 3.5 Artists' Coated (Prepared)
- 3.6 Coated Papers
- 3.7 Tissue/Tracing Papers
- 3.8 Cardboard/Artist's Board/Illustration Board
- 3.9 Watercolor Papers
- 3.10 Artists' Printing Papers
- 3.11 Asian Papers
- 3.12 Japanese Papers
- 3.13 Composite Structures
- 3.14 Wallpaper
- 3.15 Restrained Papers
- 3.16 Over-Sized Papers
- 3.17 Three-Dimensional Paper Objects
- 3.18 Fans and Screens
- 3.19 Papier-Maché
- 3.20 Globes
- 3.21 Traditional Non-Paper Supports
- 3.22 Papyrus
- 3.23 Palm Leaf
- 3.24 Parchment
- 3.25 Pith Paper
- 3.26 Tapa
- 3.27 Drafting Cloth
- 3.28 Contemporary Non-Paper Drawing Supports
- 4 History of This Chapter
Factors to Consider
Inherent Physical Characteristics of Paper
Physical and chemical characteristics determine how successfully a support will respond to exhibition and/or conservation treatments and the degree to which they may be applied.
With experience and testing, the conservator can judge approximate fiber content and anticipate the success of treatments. Exact fiber identification may not be necessary before treatment, though approximate fiber identification may be reached after considering factors such as condition, context, and dating.
Color (See also Colored Papers )
Actual color of the artifact may be a result of darkening or lightening, or tonal shift from chemical changes caused by aging, mishandling, mold, exposure to light, or conservation treatment. For example, discoloration of size can occur through degradation produced by sulfuric acid, a by-product of alum in the size. Conservation treatments may attempt to correct the above changes where there is evidence of instability or degradation. However, it may not be possible to return to the original color with conservation treatment. One may have to accept some changes due to aging or due to inherent components of paper. The object's integrity and its specific needs should give direction to conservation treatments.
Weight may be altered by the removal of soluble or reactive additives or other inherent components (i.e., lignin, acid products, fillers, starch, optical brighteners, etc.) during treatment. A change of weight is not usually thought of as a significant factor in conservation treatment.
Thickness may be altered by swelling of fibers by water or alkaline solutions during aqueous treatment and/or extreme pressure during flattening. Lack of restraint during drying can result in a more porous, swollen sheet. (AD)
Strength may be altered by chemical embrittlement due to aging, contact with acidic materials, aqueous treatment in poor quality water, highly alkaline treatment, or inappropriate bleaching methods, mechanical damage, and removal of sizes or coatings.
Strength may be altered from washing, addition of sizes, and other aqueous treatments. Washing in suitable water quality removes impurities which interrupt fiber-to-fiber bonding.
Absorbency may be reduced by the addition of transparentizing agents, coatings, or sizing (gelatin, glue, starch, gums, resins, or cellulose ethers). Sizing is added specifically to improve resistance to moisture penetration. Waterleaf (blotting) paper has no sizing or coating; fluid media will bleed into it. The addition of alum to gelatin produces a harder, less water-soluble size upon drying. Absorbency can be reduced by removal of soluble deterioration products. (AM)
Absorbency may be increased by the removal of sizing or transparentizing agents during treatment. In contrast, sizing may be reactivated during float washing (see Cohn 1982). Solvent treatments, such as the use of ethanol as a wetting agent, may increase the rate of absorbency. Very deteriorated paper may wet out immediately due to cumulative aging properties such as the breakdown of sizing or wet out unevenly due to uneven deterioration. Often the outside edges of a sheet wet out more easily and mold damage, which deteriorates size, can create uneven wetting patterns. (KDB)
Dimensional stability of a support may be altered by compaction of the fibers in some areas of the sheet (printing pressure – typeset, intaglio, woodblock, etc.), or conservation treatment – mending, lining, drying methods, etc.
Pliability may be altered (usually increased) by the presence of moisture in the environment, moisture content of the object at a given RH, sizing, or washing out impurities that interrupt fiber-to-fiber bonding. Washing alone may change prior “restraint” characteristics or prior drying characteristics. (AD) Improving pliability may be a reason to proceed with washing.
Pliability may be altered (usually decreased) by deterioration of components of the paper on aging or poorly chosen conservation treatments (see Factors to Consider: Inherent Physical Characteristics of Paper: Strength).
Surface texture may be altered by media, mechanical damage (tears, burns, creases, abrasions, stains), results of conservation treatments (aqueous treatments, alkaline treatments, lining and/or flattening methods, use of suction table, blistering during bleaching, burnishing during surface cleaning, etc.), or as the result of mounting/matting for display (overall mounting, dry mounting, etc.). For example, if the original sizing is removed in alkaline washing, the surface sheen of the paper may be altered and the fibers softened and loosened so that texture may be further modified upon drying.
Transparency, Translucency, or Opacity
An undesirable transparentizing effect may result from aged pressure-sensitive tapes, oil-based stains, and some gummed taped adhesives.
Translucency or transparency may be decreased by the removal of transparentizing agents during treatment and by lining.
Sources of Acidity
One of the factors in the deterioration of paper is the presence of acidic components resulting from the degradation of the cellulose fiber or additives in paper manufacture. The anhydroglucose units in cellulose are joined by acetal linkages that are sensitive to acid hydrolysis.
- Fiber type and quality. For example, the fibers of ground wood papers contain lignin which is chemically unstable, especially when exposed to light, and which breaks down to produce acidic components that attack the cellulose. Newsprint may be as much as 80% or more ground wood pulp. This accounts for its inferior strength and color stability. (See Mechanical Wood Pulp Papers )
- Sizing, such as alum-rosin and gelatin with alum added, may become acidic. Gelatin is stable at a pH just below neutral. Alum is an agent added to both gelatin and rosin sizing. Alum was used increasingly by papermakers as early as the 1600s to aid in sheet formation. A by-product of the degradation of the alum used in the size is sulfuric acid. If excess alum is present it will contribute to the build-up of acidity in the sheet.
- Oxidation agents. Light, heat, and pollution provide agents necessary for chemical reactions within paper which increase the free hydrogen ion (H+) supply, therefore contributing to acid hydrolysis. Ozone is an oxidizing agent, but SO2 and nitrous oxides promote acid hydrolysis. Nitrous oxides also promote ozone formation. (LP)
- Dyes or pigments: Certain colorants such as iron gall inks, and copper greens, can hasten degradation of cellulose. (See Factors to Consider: Strength)
- Coatings (i.e., gelatin, egg-white, varnishes, glues, etc. (See also Inherent Physical Characteristics of Paper: Surface Texture and Transparency, Translucency, or Opacity).
- Residues of bleaching agents will be found especially in low-grade rag (colored or dirty, worn rags that require bleaching) and non-rag pulps. Almost all early chemical bleaches contained chlorine residues, which often remained in the paper since they were difficult to remove with ordinary washing. Chlorine is highly reactive and can form hydrochloric acid when combined with moisture. This acid is also present in paper that has been bleached with chlorine as a restoration measure and inadequately rinsed in antichlors and water. Papers affected by chemical bleaching may be characterized by loss of strength and discoloration, either immediately or with time.
- Residues of chemical pulping agents (See Chemi-Mechanical and Semi-Mechanical Pulp Papers and Chemical Wood Pulp Papers)
- Fillers (See Loaded Papers)
- Other impurities
Sources of Alkalinity
- Some sources of alkalinity include residues of chemical pulping agents, sizing, coatings, fillers, water used in the papermaking process, pigments, deacidification and alkaline bathing, and some bleaching treatments.
Heavy Metal Ions
- Some transition metals, especially, copper (Cu), iron (Fe), cobalt (Co), manganese (Mn), and zinc (Zn), may catalyze the degradation of cellulose in the presence of oxygen or moisture (Shahani and Hengemihle 1986). These metals can be introduced into the paper from the fiber source (wood, linen, etc.) which may contain trace elements from the ground in which it was grown, or by the equipment, water and chemicals used in paper manufacture (see Factors to Consider: Sensitivity of Paper to Its Environment) and by some conservation treatments. Their presence can cause problems in paper as it ages and is exposed to mold, high relative humidity, light, and pollution, and some conservation treatments (e.g., oxidative and reduction bleaching).
Sensitivity of Paper to Its Environment
The environment is one of the most important factors in the survival of works on paper. The major elements of the environment that affect paper's longevity are light, relative humidity, temperature, airborne pollutants, and housing materials.
- All wavelengths of light, including ultraviolet and infrared radiation, affect various components of paper (cellulose, hemicellulose, lignin, pigments and dyes, sizing, etc.). The mechanisms are complex (See Feller 1964). Ultraviolet radiation and the violet end of the visible spectrum can contribute the energy needed to initiate direct or indirect deteriorative chemical reactions in paper, especially when oxygen is present. These reactions also occur in the visible range. The results include color changes (fading, darkening) or actual structural breakdown of materials (Banks 1989, 80). The extent of photochemical deterioration depends upon the intensity of radiation, wavelength, and length of exposure.
Because paper is hygroscopic, changes in relative humidity (RH) affect the actual resultant moisture content of the paper (equilibrium moisture content or EMC). It is not feasible to routinely measure and control the actual EMC of individual works so ambient RH is measured and controlled instead (Banks 1989, 80).
- High RH, in combination with warm temperatures, promotes the biological deterioration of paper, encouraging the growth of mold or fungi, foxing, and/or insect attack. High RH also causes dimensional change, planar distortion, breakdown of paper size, and loss of paper strength. Rate of acid hydrolysis reaction increases in high humidity conditions; this phenomenon becomes increasingly significant with high acid content collections.(LP)
- Fluctuating moisture content generally causes stress to fibers as they alternately swell and contact. There is a lack of good information on the effects of cycling on both individual materials and composites; cycling RH may accelerate aging (Banks 1989, 81).
- Extremely low RH can reduce the flexibility of paper and cause dehydration, shrinkage and embrittlement of the specific fibers. It is not yet known, however, if for long-term permanence the presence of a high EMC is not more damaging than an extremely low RH (e.g., desert conditions).(AS)
The rate of chemical reaction doubles with a 10°C increase in temperature. Different papers have different activation energies, derived by the Arrhenius equation, which make their rates of chemical reaction extremely difficult to calculate. Lower temperatures will slow deterioration. Biodeterioration will also be reduced. Excessive heat causes yellowing, drying and embrittlement of paper and may cause an increase in biological activity. Temperature also has an indirect effect through its influence on RH and equilibrium moisture content.
Air pollution, largely from the burning of fossil fuels, contains acid forming components in the form of solid particles and gases.
- Particulate matter (particles large enough to settle out and cause soiling); dust and oily grit may be acidic, soil paper, weaken it by abrasion, provide nutrients for mold and insects and may contain traces of metals (See Chemical Stability: Heavy Metal Ions). Fungal spores are also carried in airborne dust.
- Smaller particulates may include “acid dust,” comparable to “acid rain,” which could cause chemical deterioration of organic materials such as paper (Banks 1989, 82).
- Gaseous pollutants include gases (SO2 and nitrous oxides which are a complex system of several nitrogen-based gases) that form acids in the presence of moisture and the oxidizing agent, ozone. These pollutants increase the acidity of materials that absorb them, thereby increasing their rate of acid hydrolysis and/or hastening their oxidation (Banks 1989, 80).
Paper is a good absorber of many types of organic vapors and liquids when exposed to them. Acids are transmitted into the primary paper support from prolonged contact with acidic housing materials (wood, ground wood pulp paper and cardboard, unstable plastics, acidic adhesives) although, “apart from sulfuric acid, it is not known what the migrating acids in paper are....The chances of a solid migrating are less than for liquids, but gases can migrate very easily and aging organic materials produce a variety of volatile materials” (Daniels 1988, 95, 97). This acid will build-up over time and, like internally generated acidity, it will discolor, weaken and embrittle the paper support. Typical visible problems observed include matburn and discoloration from the transferred pattern of wood shingle, corrugated cardboard backing, newspaper clippings, etc., and overall darkening or edge darkening from poor quality boxes, folders, mats and/or frames. (See also Weidner 1967.)
Protection against air pollutants, transmitted acids, etc., is provided by housing/storing objects in neutral atmospheres, in direct contact with clean, acid-free materials (near or above-neutral and with constituents that ensure permanence), and by using adhesives which remain reversible upon drying and contain no impurities.
In showcases and other enclosures, natural or synthetic materials, unsealed woods, treated fabrics, formaldehyde, or other materials can injure by vapor or contact. Some materials that have been observed to cause problems include wood, resin-based paints or adhesives used in laminate boards, dyes and finishes used on textiles, adhesives used in construction, etc. (See Padfield 1982; Miles 1986; Ellis 1980).
Alteration of Paper Support upon Aging
Discoloration of cellulose.
Fading or color changes of dyes or pigments.
Yellowing and embrittlement from oxidation of resins, oils, or waxes used as sizes or transparentizing agents. This discoloration and embrittlement may be irreversible since removal of discolored component may drastically alter transparency or feel of sheet.
Embrittlement, due to shortening of polymer units (cellulose, hemi-cellulose and lignin) is caused by oxidation or depolymerization by hydrolysis; embrittlement of tranparentizing agents, sizings, or coatings; or presence or breakdown of other components of paper sheet.
Discoloration of sizing.
Stains, particularly foxing.
Physical damage results from handling, accidents, poor quality storage and housing, including matting and framing. Natural physical weakening and embrittlement of some papers upon aging makes them more susceptible to physical damage.
Potential Alteration of Support During Handling
Stains, discoloration, oxidized finger prints.
Tears, folds, creases, splits, holes, losses.
Potential Alteration of Support During Conservation Treatment
Change in pH: acidity increase, alkalinity resulting from neutralization or buffering.
Introduction of heavy metal ions due to wash water impurities.
Possible removal of ions due to “ion-hungry” wash water.
Oxidation of fibers (oxidative bleaching).
Changes in optical/aesthetic qualities (color, luster, translucence, opacity, reflectance).
Mechanical changes to paper surface (abrasion, compacting, lifting of fibers, skinning, local or general flattening of texture, surface or interior “gritting” from crystallization of alkaline solutions, i.e., calcium carbonate). (AS)
Changes in local or general permeability to aqueous and nonaqueous solutions and in sensitivity to atmospheric humidity.
Alteration of sheet thickness by change in laminar structure (linings, backing removals, mends).
Change in flexibility.
Addition or removal of sizings, fixatives, coatings.
Change in dimensions from aqueous treatments.
Relationship of Media to Support
(See Media Problems)
Media may discolor and/or degrade paper (e.g., highly acidic media like iron gall ink, verdigris and acidic collage materials; oil paint and oil binder of some printing inks).
Media may protect paper by buffering against acidity or forming physical barrier against light or acidic materials.
Degradation of support may physically endanger media (e.g., shrinkage, expansion, wrinkling, or mechanical damage of paper causing loss of media).
Degradation of support may chemically harm media (e.g., effect of acidic paper on pH-sensitive pigments in dry state or during aqueous treatment).
Change in color and tonal relationships of media and support due to discoloration of support (darkening, yellowing, bleaching, fading or color change of dyes and pigments, stains).
Compatibility of paper and media (e.g., toothed surface will trap powdery media like pastels and charcoal).
Compacting of paper due to pressure of printing techniques or resistance to moisture by media may cause local differences in absorbency of sheet and of dimensional response.
Treatment Variations: Support Types
Traditional Western Papers
- The increasing mechanization of paper production had a compromising effect on paper quality. For example, the Hollander beater, introduced in the 1600s, chopped the fibers into shorter lengths. The early stampers, by contrast, rubbed, frayed, and spread (fibrillated) the long fibers. Paper made from fibers beaten in the Hollander is not considered to be as strong as that made from rags beaten in stampers; it is shorter fibered, less fibrillated and therefore may be weaker and less durable. The Dutch added more sizing which compensated for short fibers and gave strength.
- Handmade rag paper originally had a deckled edge with irregular folded edge flaps and edge cockles; in many cases the deckles have been trimmed. Early rag papers often show marks or fine, striated creases on the back from being draped over a rope to dry. These creases (called backmarks) are of historic interest. If the creases are removed during treatment, gaps may occur in design areas. Early rag papers may be a wide variety of off-white colors. This range of possible original colors should be considered in planning conservation treatments.
- Linen rag papers tend to retain papermaking and printing characteristics even after water treatments if carefully dried. Cotton rag papers do not retain the impression of printing after washing as well as linen papers. They do, however, retain impressions much better than papers made from cotton linters or wood pulp. It may be difficult to remove distortions from rag papers.(AD) As each sheet of handmade paper differs one from another, on should respect the integrity of the sheet and its subsequent use. Care should be taken to preserve the deckled edge and back marks.
Mechanical Wood Pulp Papers
- “The presence of lignin is indicative of a chemically unstable paper. Lignin promotes brightness reversion (yellowing) and oxidation of the cellulose, contributes to total acidity and readily deteriorates photochemically.... Residual lignin in wood pulp is chemically altered from its native state. Often it is less stable, and breakdown creates byproducts that can accelerate the degradation of the cellulosic components of paper” (Young and Burgess 1989, 14–15; see also Lyall 1982, 72). This increase in the rate of the degradation of cellulose accelerates embrittlemen. In the past, chemical pulp or other stronger fibered pulp has been added to newsprint to strengthen it so the web could be carried over the papermaking machine successfully. Recent developments have given mechanical pulp greater suppleness and bonding capacity using little, if any, reinforcing chemical pulp. Ground wood papers deteriorate rapidly, even when stored under the commonly accepted conditions of 68°F (20°C) at 50% RH. Mechanical ground wood pulp paper darkens (yellows) rapidly if exposed to light and atmospheric pollution.
- The preservation of ground wood paper is a difficult problem. Until the mechanism of the degradative processes is understood it will be difficult to treat valuable items with confidence (Lyall 1982, 84). The long-term preservation of these papers may not be possible. Washing to remove acidity and degradation products, deacidification, proper housing, and limited exposure to light improve chemical stability of ground wood papers. In some collections, such as archival materials, changes in paper tone and texture which result from washing, deacidification and alkalization, are considered acceptable modifications since chemical stability is enhanced.
- Bleaching (oxidative, reductive) usually lightens the color of darkened ground wood paper initially; however, darkening may occur later. (See 19. Bleaching 1988, for details.) It may also unduly brighten a ground wood paper that was never bright white.(KN) Sun bleaching may not be appropriate for lignin-containing papers; may cause darkening or random spots.(NA)
- Alkalization is a logical treatment for acidic ground wood papers, but it usually darkens, yellows, or grays the paper. The choice of alkalization treatment will have an effect on the paper color that results immediately after treatment. Some research (e.g., Lyall 1982, 83) suggests that alkalized paper will show less cumulative darkening after aging than non-alkalized paper so that both will end up about the same color. Choosing not to alkalize means that there will be no neutralizing of the inherent acidity. Washing before alkalizing will lighten the paper a great deal. Not only does this counteract the darkening associated with the alkalizing, but it also addresses the acidity.(CS) Some conservators feel that the alkaline buffer may get used up quickly in an acidic, reactive ground wood paper and that the benefit of alkalization may last only a few years.
- Photochemically induced yellowing of ground wood pulp paper has been shown to be caused by light of wavelengths 355 to 400 nm (Lyall 1982, 84). To minimize yellowing, exhibit with UV filters at low light levels for a restricted period of time.
- Encapsulation in polyester can preserve newsprint items and manuscripts which will be handled. If alkalization of the paper support is not part of the treatment before encapsulation, some conservators feel a sheet of alkaline paper should be inserted behind the object inside the polyester film. (See Shahani and Hengemible 1986 for considerations regarding encapsulation of modern papers and insertion of alkaline paper sheet.)
- Housing in buffered board provides neutralization and improves chemical stability.
- Reduction of temperature and maintenance of constant relative humidity may delay deterioration.
- Material on ground wood paper (e.g., newspapers, periodicals, some books) can be microfilmed as an alternative to preserving the original. Microfilming is not an acceptable solution for works of art or manuscripts on ground wood pulp paper. Although microfilming, photography, or photocopying may be done to reduce the handling of archival materials.
- New technologies may provide future preservation options.
Chemi-Mechanical and Semi-Mechanical Pulp Papers
- “Little specific information is available on the chemical effects of Neutral Sulfite Semi-Chemical (NSSC) residual lignin on paper permanence, but the stability of paper made from this type of pulp has been investigated...(A) calcium carbonate buffer may improve stability....In the absence of buffering, its stability may be no better than that of thermo-mechanical wood pulp” (Young and Burgess 1989, 15).
Chemical Wood Pulp Papers
- Since there is a wide range of chemical wood pulp papers, inherent stability can vary.
- Kraft paper is observed to deteriorate rapidly in some cases, but often is seen to have surprising strength, possibly through the introduction of borax, either to the paper itself or to the adhesive used in conjunction with contemporary kraft paper tapes.
Alum-Rosin Sized Papers
- Deterioration of papers that are alum-sized vary greatly and is not always detectable in papers with alum added to gelatin.
- “While alum is not a particularly strong acid, in the presence of certain other substances it can assume a greater strength...Excessive alum, in the form of aluminum sulfate, may react with chlorides present to form aluminum chloride (AlCl3), which in the presence of moisture and heat, will form hydrochloric acid (HCl)...” (Roberts and Etherington 1982, 9).
- Rosin is known to darken easily from exposure to light, elevated temperature and low relative humidity; this sizing appears to become quite brown if exposure is prolonged.
- Alum-rosin size was often applied to very thick nineteenth century Whatman papers. Recently examined samples showed low surface pH, however, inherent strength still appeared good.(SB)
- Reducing the darkening of the alum-rosin sizing is difficult. Until it is known how discoloration develops in this sizing and whether existing bleaching methods effectively prevent its recurrence, it is not known whether such treatments will provide anything other than short-term cosmetic effects (Perkinson 1986, 8).
- Washing alone may significantly improve the darkened appearance of alum-rosin sized paper. If these papers are housed properly and exhibited with UV filtration, darkening may be reduced for some time.
- Alum-Rosin sizing increases the light absorption of paper in the 330–440 nm region of the electromagnetic spectrum. Rosin-sized papers also yellow in natural light. This may be a contraindication to light bleaching.
- If resizing is thought necessary, use of synthetic products or gelatin might be considered.
- Some solvents affect sizing, cause tiding, and change absorbency of paper. This can be a problem, particularly with local treatments.(LP)
- One of the most difficult tasks for a paper conservator is to determine the original color of the paper. Important elements to consider include aesthetic considerations, close examination of the paper, comparison with similar works, interaction of the media and paper, analysis of paper fibers, and paper colorants. (For a specific application involving these considerations see Perkinson 1986, 1.)
- Unstable pigments and dyes may fade in light Exposure to UV light over an extended period of time may change the structure of an optical brightener so that it no longer functions as a UV absorber and cause the paper to appear yellow.
- Consequences of treatment procedures (washing, alkalization, stain removal, etc.) must be carefully considered. Unstable pigments (usually organic) and dyes may change color. For example, Prussian blue, a known colorant of gray-blue and gray-green papers from the 1770s, can be decolorized by alkali solutions.
- Optical brighteners may be unstable to some wash solutions and bleaches; organic solvents used in tape removal, etc., may remove or dissolve optical brighteners.(KN) Optical brighteners can also change solubility over time.(KDB)
- To verify the presence of an optical brightener examine under an ultraviolet lamp. To identify the fluorescing species use comparison sheets of known brightness, analyses, and spot tests.
- Water and solvents may also remove color additives such as a contemporary paper dye. Tidelines are easily formed in colored papers with local solvent treatments.
- Surface color can be adversely affected by overly vigorous surface cleaning due to abrasion or changes in optical qualities which alter visual perception.
- Loss of calendered surface. Surface abrasion or burnishing will leave visible marks on a calendered surface.
- Aqueous treatment may cause alteration of the compacted, often shiny paper surface through swelling of the paper fibers with moisture contact. Characteristics of the calendered surface may be difficult or impossible to reintroduce.(NA) The high pressure and hard surfaces used in the original papermaking process are needed to recreate the characteristic surfaces.
- If media permit, surface character can be reestablished with a variety of techniques: drying face down on glass with pressure from above, spraying with very dilute gelatin solution and drying face-down on silicon release or polyester film, or burnishing (directly on object or with an interface to increase/decrease gloss).(CS) Where media allows, flattening in a press between rag board may be more successful in restoring surface than pressing with blotters under weight.(LP) It may be possible to use a barrier sheet such as silicone release or glassine.
- To reduce surface dirt, use grated white vinyl eraser, lightly rubbed. It may not be possible to remove all surface grime.(AS)
- Rapid absorption of liquids; increased penetration.
- Decrease in strength. The strength of paper is mainly a result of fiber-fiber interactions; pigment particles between the fibers will interfere with fiber interactions (Casey 1981, 1528). Thus, the addition of fillers weakens the sheet structure. In sheets of the same basis weight, the sheet containing filler will contain less fiber than the unfilled sheet, and will be weaker.
- Alkaline loading materials, such as calcium carbonates, may act as a buffer. This explains the relative good condition of loaded papers made from poor quality fibers.(LP)
- Deep creases, folds, and dents to these papers often result in a distinctly different color along the line of damage. (CS)
- Water stains loaded papers very easily (e.g., gray Oriental clay-loaded papers favored by Matisse for lithographs).(KN)
- Lack of internal and surface strength may cause problems with hinges shearing off and mends and infills may be difficult to remove. Moisture must be kept to a minimum in the above treatments to avoid tidelines and staining.(TF)
- Loading of calcium sulfate may be lost in repeated cycles (five) of float washing/drying (Cohn 1982; Daniels 1986, 71–72). Loadings in papers used in modern posters can be lost in water washing.(KDB)
- See also Japanese Papers
Artists' Coated (Prepared) Papers
- Artists' coated papers may exhibit abrasion or burnishing of surface, flaking of ground (caused by drying out of binder and aggravated by an excessively dry environment), inability of coating to withstand the dimensional response of paper to fluctuating relative humidity, creasing and folding of paper.
- Stains form easily in the absorbent ground layer which limits use of aqueous treatments to reduce stains or discoloration. (NA)
- If the coating is heavy and applied to only one side of the sheet, humidity fluctuations over time may result in draws, undulations and bulges that are impossible to remove. Heavy inks on top of the coating magnify the problems (e.g., silkscreens by Andy Warhol and Josef Albers).(CS)
(See Coated Papers).
- Some have little strength. Can be very stiff and/or brittle.
- Zinc oxide and titanium dioxide are known photosensitizers of cellulose.
- Coated papers are generally very sensitive to and easily damaged by moisture or humid conditions.
- The surface of a coated paper is easily damaged or stripped. Scratches and abrasions scar and dull or burnish the finish.
- Heavily coated papers or embrittled coatings can crack or flake and the coating can pull away.
- The surface can absorb extraneous material like resins or oils from adhesives. This causes embedded stains which are difficult to remove (Baker, van der Reyden, Ravenal 1989, 1).
- Inks or paints applied to a coated surface may not bond well, resulting in cleavage. For example, Andy Warhol's silkscreens.(CS)
- Options for the conservation treatment of coated papers are limited. The use of dry cleaning agents or solvents to remove dirt and stains can lead to cracking and flaking of the ground or to changes in surface appearance (color, refractive index or reflection change) (Baker, van der Reyden, Ravenal 1989, 1).
- Coated papers that have become wet will fuse together as they dry. If adequate steps are not taken to separate and treat the material when it is still wet, permanent damage can result Freeze-drying has proven especially useful for some, but not all, types of coated papers (Parker, 1989, 4–6,8).
- Solvent treatment can cause ring stains.
- Washing can darken clay coatings. Also, characteristic surface gloss is altered by wetting; this is difficult to recreate through conservation treatments. (NA)
Western Tissue Papers
- Glassine tissue: Acid-process glassine is, of course, inherently acidic.
- Very sensitive to water, expands greatly when wet and distorts readily.
- Neutral glassine may be suitable for temporary interleaving purposes though sharp edges may be problematic near fragile media on paper supports and it may become more acidic in time. It is very reactive to moisture, distorting severely and is dimensionally unstable with environmental cycling. Nevertheless, many collections prefer to use glassine because it is “see through.”(NA)
- Tracing papers in general react very dramatically to moisture changes; they expand, cockle and wrinkle easily. Oil/resin prepared tracing papers are less reactive, however, than natural tracing papers which have a greater capacity to expand with moisture. Cockling of the support around pigment wash areas may be an inherent characteristic of some works on tracing papers.
- With aging, prepared tracing papers may become extremely brittle and discolored because of the presence of impregnates, especially when stored in a poorly regulated, acidic environment. (SRA)
- Translucency makes the addition of unobtrusive hinges, mends, fills and linings problematic.
- Adhesion of starch pastes are problematic with some impregnated papers.(LP)
- Storage: Large works on tracing paper may require rolled or folded storage; this may cause problems of access, especially when the support is deteriorated. The ends of the rolls are often damaged.
- In the case of tracing papers that have impregnating agents, treatments can interfere with the original appearance and remove material evidence. Some solvents may cause loss of translucency on some papers as a breakdown of impregnating agents (Baker, van der Reyden, Ravenal 1989, 10). It is suggested that treatments to these types of papers should be kept to a minimum. Conversely, natural tracing papers that have been transparentized by extensive beating of the fibers can withstand extensive treatment (e.g., washing, bleaching, etc.) and will dry without alteration to the surface.(SB)
- Modern natural tracing paper is much stronger than one might expect. It can be manipulated when wet, if it is well supported. Soaking in water does not always completely relax creases, but it may to the extent that the work can be flattened. The object may also be relaxed until limp using vapor from an ultrasonic humidifier.(NA)
- Mending with Japanese paper and wheat starch paste and/or methyl cellulose is usually very successful but, because of the tendency to distort with moisture, only small areas should be worked on at a time. Heat-set tissue (e.g., Rhoplex on paper base) and BEVA mends have also been used. A slight change in appearance may be considered acceptable since it is often unavoidable. The Library of Congress (LC) heat-set tissue works on some tracing papers and when applied with ethanol rather than heat or in combination with heat is almost invisible. More invisible mends can be obtained with a “gossamer tissue” coated with Klucel G developed by F. Mowery. (On the other hand, the Mowery tissue does not offer as much support as the LC tissue.[CS]) Tissue with BEVA 371 or Klucel G applied using solvent instead of heat works well.(CS) The challenge of making mends, fills, etc. unobtrusive may be met by using the optical properties provided by placing a sheet of opaque paper or mat board behind the tracing paper.(SP)
- Backing methods include the use of traditional “wet lining,” heat-activated systems, and solvent activated systems. (See Bachmann 1983 for a summary of the literature to that date.) For the wet lining of nineteenth century tracings, thin Japanese machine made roll papers and very dilute wheat starch paste are recommended; both tracing and roll papers have the same dimensional properties (Nicholson and Page 1988).
- Be aware that solvent treatments on impregnated papers (especially with ethanol and acetone) may alter original tracing paper.(SP)
- Drying and flattening are very important treatment steps for most tracing paper supports which are thin and dimensionally unstable. Successful methods may include the following.
- Flattening with considerable weight between hard surfaces (e.g., rag board) has been successful.(NA)
- Stretch drying on a screen (mizubari or karibari): moisture and friction bind the primary support between a protective wet-strength tissue on the face and false backing of a suitable Japanese paper; a line of paste is then applied around the extended edges of the Japanese paper. The object is adhered, face inward, by the pasted edges to a Japanese drying screen (also called karibari) or other board. Once dry, the object is dismounted and the false backing and protective tissue are peeled away (Keyes 1984, 101–102; Futernick 1984, 68). Not suitable for objects that are weak, brittle, or damaged by tears or weak fold lines.
- Friction mounting: Combines the use of a false backing (described above) with pressing in a press or between plate glass sheets and under weights. Far less moisture and friction contact are required in this method so that moisture can be reduced to a minimum for vulnerable objects. “Vapor humidification in a chamber or contact humidification between moist blotting paper provides enough moisture for successful friction mounting” (Keyes 1984, 102–104; Fletcher and Walsh 1979, 122–124). Friction mounting may also be undertaken without using a press; sometimes thick felts will provide adequate pressure. (SRA) Felts are useful because they conform to the surface irregularities of sharp creases often present in tissue paper which has previously been folded. (SP)
- In all cases it is important to match the grain directions of the original support and the secondary mounting papers.
- Friction mounting variation: Place a totally relaxed object face-down onto glass; smooth, thin porous Hollytex on top of object; a blotter extending beyond the glass above the Hollytex; glass and weights. The protruding blotter allows moisture to be removed from sandwich without need to open package risking the formation of cockles. (CS)
- Drying against Mylar or Parafilm to encourage a smooth surface. Watch for mirroring.
- Some transparent papers can be successfully flattened on the vacuum suction table after first thoroughly humidifying them. Care must be taken to avoid “blotter impression” on these thin papers. (CIM)
- Hinging: See Matting and Framing. One successful method for hinging lightweight papers is to make tiny cuts in the “attachment edge” of the hinge and remove alternate segments, creating a “tiny comb.” Paste only 1 mm of the comb and attach it to the object. Attach hinge to back board 5 mm above the top edge of the object. This method solves the problems posed by the transparency and dimensional instability of tissue and tracing papers (Futernick 1984, 68–69). An alternate hinging method uses hinges made of Hollytex Lite prepared with dilute Lascaux 498–20x or 498–HV which can be reactivated with appropriate solvents or with heat. (AM) Non-impregnated tissue paper may be hinged by application of heat-set tissue and detached with solvent. (SP) For tracing and other papers that are very slick, very calendered, etc., small squares of double-sided tape may be used instead of traditional hinges. This has mainly been for exhibition purposes: the tape has been easily removed after a few years, however long-term stability, etc. is unclear. (KDB)
- Polyester film (Mylar) encapsulation is also a satisfactory way to support tracing paper inside mats. Encapsulation provides physical support, however, be aware that Mylar has strong electrostatic properties and that tracing paper may be torn easily while working. Encapsulation is not recommended for tracing paper with graphite media. (SP)
- Preserve through environmental control. House in special mats to prevent mishandling. Matting these papers can create great danger; the paper can be sucked upwards with the opening of the mat. See Matting and Framing
- Transparentizing material is original and its removal is ethically, as well as practically, questionable. Solvent extraction of transparentizing material such as oils is a debatable treatment, which can remove darkened oils but leave paper opaque. (KN) The paper after oil extraction may be discolored and embrittled. (TF) Removal of transparentizing materials is sometimes necessary if the image is to become visible again. Have high-quality photographs made before extraction. Explore the possibility of adding an archival quality impregnate after removal of the discolored one. (CS)
Cardboard/Artists' Board/Illustration Board
See Backing Removal.
- Delamination of pasteboards, especially at the corners and around the edges, is a common problem. There is also a tendency to separate when damp. Breakage due to the combination of acidity and inflexibility may also occur.
- Early pulp boards tend to be soft and spongy.
- Thick boards may distort with moisture and are difficult to flatten.
- Artists' Illustration Board: Acid migration from a poor quality lignified core board will discolor and embrittle the better quality facing paper which bears the image.
- Readhere delaminating pasteboard sheets where desirable.
- Filling losses: Cardboard often has losses with jagged cross-sections. Japanese tissue or blotters can be shaped to fit one layer of the irregular edge of the cardboard and adhered with wheat starch paste. Another layer of paper may be torn to fit into the next shape presented by the object. Repeat until the front of the cardboard is reached. Finally, apply a larger piece of strong tissue over the top of the fill and extend onto the object enough to cover the break line. Tone the laminates or uppermost layers as necessary. (CS)
- In some cases, the use of paper pulp may be the best way to fill a jagged loss. “Back” fill with Japanese paper for added strength, especially with corner losses. (CIM)
- Hinging: See Matting and Framing. Hinges attached to the top edge of the artwork may be pushed through slits cut in the back board so that secure attachment can be made on the back of the mat board (Futernick 1984, 69–70). Use a sink mat to create a ledge below the object for it to sit on. Add a “fence” to the other three sides so they protect against swinging of the heavy object and against physical damage to the laminate edges.
- One must consider the importance of the board to the historic/artistic integrity of the object versus the need to remove the board for the long-term preservation of the image and/or primary support. Separation of the primary support from the secondary core if necessary/possible is tedious, difficult, and time consuming. The loss of structural integrity to illustration board may be offset by the risk to a thin primary support by an embrittled secondary support. See Backing Removal.
- Commercial watercolor board: Survival of the facing paper depends on the quality of the core. Acidity from the cardboard core can migrate to the facing paper, causing embrittlement and discoloration. See Cardboard/Artists' Board/Illustration Board.
- Casual selection of watercolor papers by some twentieth century artists practically guarantees the use of machine made paper, sized with alum-rosin. See Alum-Rosin Sized Papers.
- The potential for cockling is a characteristic of all papers; it is usually a function of the thickness of a sheet (see Thickness under (Inherent Physical Characteristics of Paper) with thinner papers being more susceptible.
- Distortion of technical evidence with change in dimensions during aqueous treatments: the size of a watercolor, taken before treatment, may be a fraction of an inch larger than the standard dimensions of nineteenth and twentieth century commercially available watercolor papers. “By wetting and stretching individual sheets prior to painting, the artist would inadvertently increase their dimensions by as much as one-half inch, a size they retained when freed from stretching” (Walsh 1987, 54). Further change may result depending on drying/flattening methods selected.
- Alteration of original technical evidence can result from flattening of cockling that occurred during execution of the watercolor. (NA)
- Technical evidence may also be lost when remnants of “watercolor block” binding material along the outer edges of a sheet are inadvertently removed in treatment, or if a secondary board mount, to which the primary support was attached before execution of the watercolor, is removed since brush strokes often extend over the paper edge onto the board. (NA)
- Washing and drying treatments can increase/decrease the surface texture of some watercolor papers if not accomplished carefully by an experienced conservator.
Artists' Printing Papers
- Plate paper/copper plate paper is vulnerable to mold and foxing stains. Grime is easily embedded into the paper surface.
- Vellum has a very nonabsorbent, glossy printing surface. The printing ink may not penetrate the surface resulting in flaking of the media, particularly with fluctuations in ambient relative humidity/moisture content. Ink may be easily abraded, especially at the high points of a cockled sheet.
- Japanese Papers: Gauguin is known to have printed some woodblocks in black ink on a support paper, and then covered the support (and printed image) with a thin tengujo (kozo) veil. He recut and printed the block on top of the tengujo. It is almost impossible to see but important to know about before treatment (Dwan 1989, 9).
- Nineteenth century prints on Japanese papers often show a shiny, burnished area from contact with the metal plate during printing; this contrasts beautifully with the matte, unprinted and unpressed margins. The burnished area can easily be damaged by abrasion, distortion, or swelling during aqueous treatments (Dwan 1989).
- Plate paper/copper plate paper: Dry cleaning may be difficult. Plate impression may be lost during treatment. (AD) Crisp, fresh plate impressions in particular may be affected. However, sometimes a squashed or barely visible platemark may be revived somewhat through aqueous treatment. (NA)
- Blind stamps, printers' chops, and other embossed marks can be reduced in crispness during aqueous treatment. The finer and more detailed the stamp, the greater the tendency toward softening of detail. (NA)
As in any industry, the quality of paper manufacture varies greatly. Many Japanese papers are in beautiful condition, but may have discolored with age and/or developed foxing. This can be due to the addition of mechanical wood to the pulp, impure water, iron used in the manufacturing process, alum rosin size, drying on heated metal panels instead of wood boards, etc.
- Kozo: Soft, layered structure makes kozo, in particular, vulnerable to thinning and grayness from embedded dirt and abrasion (Keyes 1988, 32).
- Hosho with kozo fibers: Because it is dipped several times during manufacture it can easily delaminate between the layers during aqueous treatment (Dwan 1989). Torinoko and Maniai-shi (gampi fibers) do the same. (YN)
- Gampi: Strong expansion and contraction characteristics are observed if exposed to fluctuations in relative humidity or aqueous treatments. They will expand and contract more than other papers. “The plate measurements of an impression printed on Japanese paper will often be two to three millimeters smaller in both dimensions as compared with those of the same subject printed on a European paper” (Boston Museum of Fine Arts 1969, 180). Because of their thinness, gampi papers wrinkle and ripple easily and repairs can often be seen. If improperly mounted they can buckle and distort dramatically, therefore, they are not recommended for backing paper. (YN)
- Traditional presentation in the West: Some Japanese papers are “gossamer-thin” and so were often mounted for protection (Nicholson 1988). (See Collé Paper). One may encounter prints attached to the mat by a thin band of paste around all the edges or laid down with the entire verso of the primary support stuck to mat board with paste or dry mount tissue. The quality of the mat board can pose a serious conservation problem; it may contain lignin, be acidic, brittle, and discolored (Nicholson 1988, 39). Mats constructed in the traditional fashion expose these papers to potential damage when the mat is opened, as they are easily sucked upwards. (CS)
- Sizing: To meet certain needs, some papers were sized with a mixture of gelatin and alum (doza). In some cases the mixture has caused deterioration of Japanese papers (Inaba and Sugisita 1988).
- Spotting: Uncleaned black bark left in the paper can cause deterioration in the surrounding area due to lignin, etc. Foxing can occur due to the manufacturing process.
- Abraded paper surface: Loose paper fibers, soiled and rolled or pilled. Cut away fiber outcroppings, “tame down” shaggy fiber projections with dilute paste or resize (Keyes 1988, 33). Methyl cellulose also works well. (CS)
- Options are limited in surface cleaning because the papers are unsized and have a soft surface. Cleaning through another piece of Japanese paper can be helpful. (SRA) Using a thick, flattened piece of kneaded eraser which is forcefully pounced straight down, straight up, again and again is also a possible method. (CS)
- Local discoloration (e.g., foxing) can sometimes be reduced on the vacuum suction table because the paper fiber network is so open. However, the same mobility of discoloration can cause haloes.
- Introduction of moisture:
- Because these papers are unsized, characteristics can be lost during aqueous treatments; however, local treatments can be successful. A. Dwan has had success retaining impression and brush strokes during aqueous treatments to remove stains by using selected alcohols (propanol) to “resist” non-treatment areas. This work is still in the experimental stage.
- Use of steam is not recommended since it can easily create tenacious translucent stains, apparently by affecting the mucilage used in papermaking (Keyes 1988, 32).
- Gore-Tex treatments have been very successful. Also, suction table treatments and humidification with blotters.
- Drying/Flattening: Their thin porous structure makes some Japanese papers dimensionally unstable and prone to wrinkles and other distortions. For stretch drying on a screen and several methods of friction mounting see Tracing Papers).
- To protect the burnished plate area of a Western print on a Japanese paper, a washed Japanese paper (that has been given a slick surface by drying it against a metal surface) is fitted to the plate area by water-tearing it. The smooth side of this “insert” is placed next to the burnished plate area on the washed and damp Western print; then a sheet of lens tissue and felts for final drying are added (Dwan 1989, 11).
- Success in drying gampi is obtained by placing it between Gore-Tex (with the smooth sides facing the gampi), sandwiching this between blotters and felts, and placed under a light weight. Brush through Hollytex to ensure contact of the gampi with the Gore-Tex. The smooth surface of the Gore-Tex retains the smooth surface of the gampi, yet allows water to be removed equally from both sides of the sheet. The light weight and light restraint of the Gore-Tex sandwich helps to retain the impression of modern Western prints (Dwan 1989, 10).
- Gampi can be dried on/or against Mylar or Parafilm sheeting to avoid problems of edge adhesion. In the past, glass has also been used as a smooth surface on which to stretch-dry gampi.
- Gasenshi is unsized and very absorbent, but weak and easy to abrade in surface cleaning, easy to skin, and easy to lose textures (prominent brush marks from traditional drying process, calendered surface, matte and burnished areas from metal plates used to print Western prints) in aqueous treatments and subsequent drying and flattening (see Japanese Papers) (Dwan 1989).
- Local treatment on gasenshi papers may cause permanent tide lines because of the white-tone from a filler (wara, a rice straw powder). This filler is very absorbent. It is probably this that moves during aqueous treatment and produces white tide lines by redeposition. Use of amylase enzymes is contraindicated because of the presence of the starch based filler (Dwan 1989).
- Resizing is appropriate for most traditional Ukiyo-e (Japanese woodblock prints) but not for surimono (a category of privately commissioned prints used for seasonal greetings and announcements on lightly sized or unsized paper) or other unsized sheets (Keyes 1988, 30). “Resizing may be considered when the print is limp and lacking its normal body, when the paper surface has been roughened and fibers are loose, when repair was extensive and the general tension balance needs to be established or when large areas have been treated with enzymes. Good quality gelatin is used in a concentration of 0.5% or less. It is normally applied in a spray, but the manner of application may be adjusted to accommodate the tolerance of the colorants present” (Keyes 1988, 33). The papers, if traditional, were sized with the mixture of gelatin and alum called dosa. Test for protein and resize with a good grade of gelatin. The size may have been applied on one side only. (JM)
- Manufacture: Generally, current standards of papermaking in China are low. Sulfurous acid (H2SO3) is used in pulping liquors, sodium hypochlorite (NaOCl) in bleaching, and the size contains aluminum sulfate. All leave damaging residues which can cause yellowness, fragility, and eventual crumbling. Some mills still produce calligraphy paper (xuan zhi) by traditional methods (Zhou 1988, 19).
- Presentation: Traditional Chinese paintings were produced on a laminated structure to give “strength and body” to the smooth, fine, thin, light paper used as the support.
- Manuscript and early printed scrolls: Mounted in the 1960s and 1970s in the West in the manner of oriental paintings, although mounting was not a traditional format (scrolls formed part of a library, not a collection of paintings). Lining and rolling was an easy option. Lined, rolled objects inevitably crack or delaminate because of the tension between the lining and the primary support. Type of method of manufacture, diameter of roll and thickness of paper and adhesive are also contributing factors.
See Japanese Papers for other notes on unlaminated objects.
Near Eastern and Indian Paper
The addition of the coating of starch and burnishing makes Indian and Middle Eastern papers difficult to treat. See Coated Papers.
- Often Indian and Middle Eastern papers are laminates or cut-outs of various pieces of paper adhered together with a very fine overlap. The structure should be studied very carefully before treatment.
- The introduction of moisture in treatment should be approached cautiously. Tidelines are a constant problem and can be very difficult to remove. For the same reason other Asian papers with starch fillers are difficult to treat.
- Using alcohol locally causes starch size to turn grey which is impossible to remove.
- Plate paper is porous and often prone to foxing and water stains.
- During aqueous treatments the collé paper layer may separate partially (discrete scattered bubbles, along edges, or at corners) or completely from the plate paper. However, there may be strong physical attachment at heavily printed areas; use caution when attempting to completely detach the collé paper. Impression quality on chine can be compromised during aqueous treatments.
- Use a suction table to control aqueous treatments and discourage separation. Use damp blotters and webbing supports to pull out the staining without separating the two layers.
- If there is no indication that delamination will occur, float washing may be used. Have the suction table set up in case it is needed. To reflatten bubbles that may appear, remove the print from the bath and leave it on blotters until the collé is almost dry. Have on hand a dilute solution of cellulose ether. Encourage the bubbles to dry more quickly than the collé paper around them by touching their tops with the soft edge of torn blotter scraps. As they dry, they will grow smaller. Do not allow the perimeter to dry completely if there is still height to the bubble. If necessary, brush a little water around the bubble's edges to keep the deformation soft and rounded. Avoid linear drying patterns, like “ledges.” When the bubble has only the faintest degree of moisture left and has almost shrunk completely, brush on a tiny bit of dryish cellulose ether, wait for further shrinkage and less adhesive tack and then tap into position with the rounded edge of a warm tacking iron. This technique eliminates the bubbles in the majority of cases. Occasionally, a bubble will not shrink enough to be tapped into place without creating wrinkles. In these cases, puncture the top center of the bubble with a titanium microscopy needle - with the fibers damper than for the other technique, so the puncture will be ragged - and continue as described.(CS)
- Readhesion may be complicated by the fragility of the thin pressed paper, the differences in dimensional responses to moisture, and on the need for precise registration. Supporting the wet chine on Mylar may assist in realignment. (NA) For reapplication of a lifted tissue, use a Mylar carrier and raking light. Have both papers and the adhesive as dry as possible. Starch paste or other adhesives can be used.(CS)
- Sometimes text overlaps the join line between papers and often there is a distinct outline of the collé paper on the plate paper, so misalignment will be very obvious.(KN) Impressions on both papers may be impossible to match.
- Use of incorrect methods and/or materials in the initial mounting may cause planar deformation, wrinkling, uneven attachment/separation, discoloration, etc.
- Objects were often lined with the intention that it would enable easy rolling. Often they were rolled image inward to protect the image. Consequently, this caused compression, cracking, etc. of the paper and media.(KDB)
- Differences in structure and method of manufacture and preparation may cause the paper and canvas to react to atmospheric changes and exposure to liquids and solvents in opposite ways (e.g., mechanical stresses, shearing and loss of adhesion).
- Stretcher/strainer mountings subject the object to more risk of physical damage by puncture, shock that leads to cracking in heavy paint layers, drawing at corners and deterioration of tacking edges.(CS)
- Physical and chemical characteristics of the attaching adhesive represent a further complication - adverse effects of aging/deteriorating adhesive (e.g., yellowing, staining, embrittlement, and decreasing reversibilities).
- Aesthetic surface changes in paper tone, texture, and flexibility associated with fabric and/or adhesive.
- Conservation treatments of contemporary works mounted to canvas should acknowledge the aesthetic significance of the artist's original mount. Consultation with the artist, curators, and/or art historians may be required before treatment.
- One option for retaining the historic format of a cloth lining while providing a more compatible and reversible support for a treated object is to provide a separating layer of Japanese paper such as tengujo between the object and the cloth (van der Reyden 1988).
- If the object is on a stretcher/strainer, one should attach a Tycore or corrugated board filler to protect the exposed back.(CS)
- Replacement of a strainer with a rigid, chemically stable support of the same dimensions is often appropriate for items mounted on a strainer. An attempt to flatten tacking edge can cause distortion in image area.(LP)
- Spot attached drawings may not lie flat. Some undulation may be expected and may not interfere with an appreciation of the drawing, but draws may be exaggerated and distortions can occur around each adhesive daub. Extreme tensions have been observed to shear and delaminate the paper (on the verso) around the daubs.
- Drawings mounted overall tend to remain in plane with their secondary support, but may suffer from lifting or bubbling.
- In addition, compound drawings may suffer disfigurement from glues, tapes, and framers' notations; from having been cut down or folded to fit into smaller frames; from removal and disposal of the secondary supports.
- Historical mounts may suffer from every sort of chemical, physical, and/or biological deterioration that the primary support is subject to.
- Adhesives can cause staining.
- Releasing primary from the secondary support may be desired if there is physical damage, extremely disfiguring distortions caused by tensions in spot attachment, the adhesive is expected to cause stains or acid damage over time, or the primary support is very delicate or weak and has not yet, but could, become drawn or deteriorated.
- In making this decision, the conservator should consider the stability of the environment in which the object will be housed and the ability to monitor changes in the object. In excellent housing and environmental conditions and with the ability to monitor the object, a conservator may choose not to alter artist's mounting methods. In the case of the Klee drawings it was decided to retain the overall character of the sheet as well as evidence of past attachment by the artist (for more discussion on this particular case see Schulte, Ellis, and King 1986, 27–28).
- If possible, reattach (or readhere) any delaminated areas using paste alone or with Japanese tissue hinges of appropriate weight.
- Reattach to the original secondary support using hinges. Hinge along all four edges over an isolating layer of lightly buffered Japanese paper (also hinged to the mat) if this is required for isolation from poor quality materials.
- If possible, use ragboard lined Plexiglas spacers rather than an overlay window mat to isolate the work from the glazing. This best presents the original mounted format for exhibition.
- In the case of collage materials, pieces can become individually damaged or cause damage to each other (see King 1978).
- If disassembly of a collage is necessary, document the object and its various parts with tracings as well as with photographs before beginning treatment. Mark every shape and have a style of marking to designate support areas versus applied areas. If appropriate, make notes along joint lines about overlap or anything else one may forget over the course of a long treatment. Collages may have applied pieces completely hidden by upper layers (e.g., R. Motherwell). Photograph extensively during disassembly of multi-layers of objects, to facilitate the study of the artist's process by art historians and others.(CS)
- Depending on the media involved, attachments can be held in place during washing by facing with lightweight Japanese paper and methyl cellulose. The methyl cellulose will not release during warm water washing but can be removed afterward with cool water applied with a swab.(DvdR)
- In C. Oldenburg collages, conspicuous masking tape tabs were used to adhere collage papers to the support. In one example, the masking tape was discolored and detaching and with the consent of the curator, the masking tape was removed and solvent used to remove adhesive from the carrier. The carrier was lined with thin Japanese tissue and wheat starch paste and readhered in the original position.(NA)
- Strainers: Papers are easily punctured, especially as the secondary and/or primary supports deteriorate, becoming weak and brittle. Breaks or tears in the edges of the secondary support may result in uneven tension and planar distortion of the primary support. Delamination of primary and secondary support (which may occur due to environmental conditions or poor materials and technique of fabrication) can also cause uneven tension and planar distortion. Papers may split due to dimensional changes of the secondary support or strainer. There may be some tendency of paper to distort by sagging into the opening of the strainer.
- In cases where the edges of the primary support have been folded around the strainer they may be damaged by tacks, nails or staples. Heavy corrosion deposits may exist at these spots. Stress on folded edges may cause rupture of paper fibers, cracking of the paper and flaking of the media. Later attempts to flatten these borders can exacerbate these problems. Abrasion of the folded edges may occur, especially as the work is slid in and out of a frame. A commonly encountered adhesive is animal skin glue. Unfortunately, more often than not, it remains voraciously strong.(CS)
- Rigid backings: Wood, masonite and cardboard panels may warp, placing the work under tension, or they may split or snap. Plastic and metal sheets may be bent or dented and glass may break. Any rigid backing to which a work is adhered overall can harden and flatten the surface texture of the laid lines, felt marks, platemarks, etc. If the work is adhered around the edges or at intermittent spots, it will undergo stress as the secondary support and the restrained and unrestrained areas of the primary support respond differently to fluctuating environmental conditions.
- False margins: Differing dimensional stabilities of the primary support and the paper into which it is inset, as well as the restraining action of adhesive layer, can cause pronounced draws or cockling. Wide or unbevelled margins which are visually incompatible may be aesthetically unpleasing. When unskillfully done “ledges” are frequently permanently pressed into the original work where the false margin overlaps it.(TF) While some view the use of false margins as a measure of protection for the edges of the work (especially one which is frequently handled) others may see extending a drawing with false margins as a violation of the integrity of the object (McAusland and Stevens 1979, 33) and as further stressing often fragile edges.(NA)
- Sometimes works on paper were “drum mounted,” that is wet out, humidified, or in some way expanded with moisture and then laid down at the edges. This, upon drying, kept the work very flat. A puncture or sudden fluctuation in RH can release tensions developed by drum mounting. Also in treatment, releasing one edge or corner could set up tension which could cause a tear or crease.(KDB)
- Contact with poor-quality adhesives and secondary supports may cause acid-transfer to and deterioration of the secondary support. Adhesives can stain papers, can penetrate them to locally change their inherent physical and chemical characteristics and may become irreversible.
- Strainers: Papers adhered to strainers may be protected against puncture by fixing a rigid backing to the reverse of the strainer and by proper framing under glass or Plexiglas. If the poor quality of the mounting materials or the deteriorating condition of the work warrant removal from the strainer, treatment options may include the following.
- Mimic original “stretched” presentation by removing primary and secondary support from strainer, removing and replacing secondary support if necessary, and then remounting the work on to a stable rigid panel of the same exterior dimensions and thickness as the original strainer. This mounting method would eliminate the danger of puncture. The solid support may be a laminate of several materials including acid-free mat board and corrugated board, paper honeycomb (e.g., Tycore), aluminum panels and aluminum honeycomb. The secondary support may be adhered to the panel only where its edges wrap around the solid support or overall by means of an interleaf layer (e.g., Hollytex, Japanese tissue, etc.) which will permit its easy separation from the solid support. Japanese paper hinges can also be attached to the edges of the primary support and to the back of the new support. (NA) If the strainer is integral to the history of the work, it can be incorporated into the mounting and framing or stored separately (the latter choice often being less desirable). (CS)
- Present the work flat by removing it from the strainer and, if necessary, from the secondary support. If the edges of the work have been folded around the strainer they may require humidification and flattening. Flattening may be complicated if the paper has stretched by “sagging” into the opening of the strainer. (NA) The artistic and historical significance of the strainer mount should be considered in determining whether or not the work should be presented flat. If the object is housed in a frame believed to be original, flat presentation should not be undertaken. (CS)
- Rigid backings: Backing removal is often necessary, either to reduce mechanical and chemical threats to the work or to return the work to its original, loose-sheet configuration. Aqueous treatment may help bring back flattened surface texture. (See Backing Removal.) If the strainer is to be reincorporated into a treated object, the object can be protected from the acids within the wood by sealing the wood. Polyester film and Japanese paper, among other things, can be used as isolating layers (van der Reyden 1988).
- False margins: After the removal of false margins light adhesive residues can still cause slight distortion of the edges. Removal of a false margin that was applied to control curl still leaves the problem of flattening which is compounded by perimeter adhesive residues.
- The logistics of transportation, storage, exhibition, photo documentation, etc. require thorough planning.
- During manipulation for conservation treatments, transport, storage and display, large-sized papers are particularly vulnerable to mechanical damage. To treat large items, experience as well as adequate space, equipment, materials, and staff are needed. Even basic treatment procedures are complicated by an object's large size and problems which may occur are likewise further intensified.
- Presentation: Factors to consider include the limited availability and high cost of over-sized archival materials and, when available, their inherent physical limitations because of their large size (e.g., buckling of over-sized ragboards, heaviness of large glass sheets, warping of oversized Plexiglas sheets, etc.) and, finally, the desire of artists to exhibit drawings in the manner of monumental paintings on canvas (Volent 1989, 31). Many contemporary artists may not want works on paper to be glazed in any way, even during travelling exhibitions. (KDB) (See Matting and Framing: Treatment Variations.)
- Storage: If possible, “Oversized works of art on paper should be framed as soon as possible to prevent damage and deterioration” (Volent 1989, 34). Horizontal storage is sometimes the only feasible system. Note, however, that it can lead to flattening and transfer of media and to permanent cockling and curling of the support. Rolled storage on a large roll or Sonotube can be a useful tool to facilitate handling. Rolling is not recommended as a technique of storage although it has been used successfully in certain problematic situations (Potje 1988). If rolling is to be used, roll the object face out. (EW) Over-sized objects, such as posters, may be encapsulated in polyester film and then hung vertically using various methods and devices.
- Multi-sheet Supports: Non-alignment of grain directions causes planar distortions: the degree to which the natural grain directions, characteristic of some of these works, are to be retained should be specified before conservation treatment is undertaken.
- “Routine” conservation treatments may be complicated because conditions such as overall humidification and even pressure are difficult to achieve on a large scale, but they are possible. (See Albright and McClintock 1982; Eckmann 1985; Fairbrass 1986; Hamm 1988; Owen 1988.)
- Historically, large posters, maps, etc., were routinely adhered to cloth linings (cloth was available in sufficiently large widths and lengths) during production or by framers or restorers. Today, the conservator may use machine made Japanese paper with its “limitless” length for greater ease in lining over-sized Western papers, especially machine made ones (extremely large blueprints, wallpaper, posters, mechanical drawings, etc.). (See Nicholson and Page 1988; Lining)
- A treatment plan should incorporate designs and specifications for mounts, storage, proper handling and future transport, and display so that the work will be protected against new problems. This may involve consultation with the artist, curator, an historians, etc. (See Matting and Framing.)
- Multi-sheet supports: Careful inspection of joints may reveal that the piece was misaligned when made; was disassembled, trimmed and rejoined; or that pieces of different images were joined. (CS)
- Some conservators advocate separating composite objects at the seam(s) and treating each section. However, detaching the overlaps of a multi-sheet support can be very risky because of differential expansion of loose versus edge-bound paper. It is difficult to predict new dimensions/alignment after detachment. General recommendations to disassemble or not are difficult to make. Each object must be individually assessed through thorough examination and testing. (For a successful treatment see Hamm 1988.)
- Causes of deterioration: Natural aging of component materials is often accelerated by poor environmental conditions and acidic storage materials, such as custom-made wood or cardboard boxes. Combined use of various materials with different reactions to temperature and humidity changes causes many problems. Sticks over time become brittle, leaves less flexible and adhesives may either dry out or, in the case of fish glue, soften in excessive temperatures. Sticks are made of materials with grain structure which, especially due to their thinness, makes them prone to shrinkage and warping. Damage to the sticks results in damage to the leaves, since the leaves are subjected to increased stress with less mechanical support. (Damage to sticks will not be considered further since it falls into the area of the objects conservator.)
- Use: As costume accessories, fans were subjected to constant manipulation, resulting in breaks, losses, tears and abrasion along the folds. They also suffered from exposure to light, dust, candle soot and other grime, oil from skin or foods, and many other deleterious conditions. As objects for collection they were again exposed to light and dust, and were often stored open, making them more susceptible to warping and sometimes impossible to reclose.
- Past repairs: Materials used in the past for repairing leaves included parchment, glassine tapes, stamp hinges, silk, pressure sensitive tapes, and various papers and adhesives. Repairs were usually made without an understanding of their mechanical effects. Past repairs were almost always applied to the surface of the leaf, rather than between its layers. Sometimes repairs were unsightly and concealed part of the decoration, and sometimes they added bulk, causing distortions and impeding flexibility of folding leaves. Some repairs have caused irreversible damage.
- New repairs and fills are made after cleaning the leaves, consolidating media, removing accretions, various residues, and old repairs. Ideally, repairs to the mount should be made between the two layers of the leaves so they will be invisible and will not cover any design areas. It is sometimes possible to use moisture applied locally to separate the leaves at breaks in the folds and then insert repairs, or even to completely disassemble, repair and reassemble the fan. Often, however, the original materials are very brittle or the media is extremely water sensitive, making it necessary to make unobtrusive repairs on the verso of the mount. Potential repair materials include thin Japanese paper, wheat starch paste, or methyl cellulose or nylon gossamer or polyester web coated with a thermoplastic or solvent-reactivated adhesive. Cleaning, repair, and replacement of missing sticks may be carried out by an objects conservator. If possible, the rivet holding the sticks together should be removed so a folding fan can be opened for treatment When this is not possible, treatment must be more limited. Simple repairs can be complicated by need for triangular supports under damaged areas and for finger pressing instead of weighting of repaired areas. It may be necessary to construct triangles of mat board faced with polyester web to support mounts which require repairs but cannot be opened out flat. Treatment of screen fans is less complex.
- Exhibition: Fans are extremely vulnerable while on display. Exhibition mounting must ensure that they are not under tension (a flat or slightly angled display is generally safer than a vertical display) and that the weakest structural area, i.e., the folds in the paper leaf, are adequately supported. Fans left open and unsupported may be damaged by irreversible warping of the sticks and flattening of the leaf. Mounts should be ramped to follow the gradual rise of the sticks toward the guard on the right and may be pleated to support the folds. It may also be helpful to secure the sticks to the mount with, for example, an interlacing ribbon of polyester web, and provide a support for the head of the fan, where the sticks are rivetted together. Screen fans may also require specially designed mounts to protect and support them (Maxson 1986, 33–38).
- Storage: If a fan is stored closed it will inevitably be subjected to the wear and tear of opening and closing whenever it is examined or displayed. Many conservators, however, feel this is less damaging than the irreversible warping of the sticks that often occurs during long term storage in the open position. Each fan should be considered individually. Closed storage is recommended unless precluded by extremely brittle leaves, flaking media, three-dimensional decorations (sequins, beads, etc.), extremely warped sticks and mounts, or repairs that prevent closing. To avoid abrasion at the folds, the closed fans, wrapped in acid-free tissue, can rest on their guards with padding material around them to keep them secure and correctly closed.
- Problems include hinge failure, punctures, tears and splits, distortion due to humidity fluctuation, media flaking, and cleavage between layers.
- Major repairs should be undertaken by a specialist trained in screen and scroll mounting. Remedial repairs, consolidation of media, reattachment of layers, and mending of tears and punctures may be attempted if not too severe or structural. A portable suction disc has been used to pull sunken puncture areas into place.
- Traditionally made papier-mâché articles should be kept in the same environmental conditions as wood since they share the same major problems – splitting and warping due to extreme fluctuations of relative humidity. In high relative humidities or with the application of moisture, varnished finishes are susceptible to bloom. With time the varnish darkens. Extreme care is necessary in treating varnished surfaces since the paint and gilding is often very vulnerable. In proximity to direct heat the surface may peel. Layers sometimes delaminate. Contemporary works may be less rigid and more “paper-like” and may require the environmental conditions generally recommended for works of art on paper.
- Delaminating layers can be readhered with wheat starch paste or methyl cellulose.
- Fills can be made using paper pulp mixed with dilute wheat starch paste or methyl cellulose. (LG)
Cast or Molded Paper
The many variables which can affect the finished product produce many possibilities for inherent problems.
- Pulp source: Cotton rag or linters are the most common fiber stock, either purchased as pre-processed blocks or sheets or pulped from rag paper or by the artist himself. Less conventional pulp sources include fabric remnants, plant materials, and miscellaneous papers such as brown paper bags or toilet paper. Some of the materials used may invite future attack by mold, bacteria, or insects. Cast shapes will be stronger if made of long fibers. Pre-processed cotton linters are sometimes insufficiently beaten. As a result the fibers may not be well fibrillated, inter-fiber bonding will be weak, and the finished work will have little strength. Repulping pre-formed papers also produces works with less strength because the fibers, already cut and beaten to make the sheet, are further shortened. Sometimes foreign elements such as glass, wire, etc. will be added to the pulp slurry. Their future degradation or mechanical interference with inter-fiber bonding can weaken the work.
- Additives: Paints, dyes, dry pigments may be added at any stage, and can have varying degrees of stability. The same can be said for sizings, such as starch, gelatin, cellulose ethers, and commercial sizes (e.g., Aquapel, Hercon 40). Some sizings also cause vulnerability to mold, bacteria, and insects.
- Water quality will affect the longevity of any paper support.
- Pulping method: The Hollander beater will produce the best quality pulp. A kitchen blender will cut and not fibrillate the fibers, so the resulting work will have less strength. Preprocessed dried pulp is simply hydropulped (i.e., mixed with water in an agitator such as a modified washing machine). Variables in beating include: fiber to water ratio; beating speed and time; sharpness of beater blades and their proximity to the bed plate. The pulper, vat, and utensils can be sources of foreign materials, such as trace metal particles which can lead to rust and foxing.
- Forming process: The two main methods are a) pouring pulp into a mold and b) forming a wetleaf upon a mold and then modifying the wetleaf on the mold or after couching. Examples of mold materials include tin, wire, plastic, latex rubber backed with a plaster mother mold, etc. A vacuum process may be used during casting. Coating preformed materials (e.g., string, paper strips) with paper pulp is another possibility. The mold or substrate may be another source of foreign materials such as trace metal particles.
- Drying: Works may be restrained or allowed to warp during drying. This may affect their future response to humidity changes. Possible drying methods include air drying; pressing followed by air drying on a number of surfaces including felts, glass, wood, metal, or the mold itself; heating; vacuum drying.
- Surface treatment: The dried work may be sanded, burnished, stamped, carved, painted, or coated with a varnish or acrylic medium. Other objects may be attached to the surface.
- Conservation: Because of the great potential for inherent vice and the often limited treatment possibilities, external factors which may cause deterioration must be carefully controlled. Humidity must be kept low enough to prevent mold growth. A stable humidity level will help prevent the cockling and warping that may result from the different moisture sensitivities of the various materials combined in the work, and can minimize delamination to which discreet layers of different materials may be prone. The chosen humidity level must take into account the requirements of any non-cellulosic materials included in the work.
- Possible treatments include surface cleaning; local stain removal using poultices; consolidation; and repair of mechanical damages. Mounting, matting and framing methods must provide adequate support and depth for the work. For example, stronger hinges of non-woven polyester with synthetic polymer adhesives and contoured backboards might provide the support that is needed.
Many variables affect the character of the embossing.
- The plate: May be one of those mentioned above, or a less common type, such as cement, plaster, etc. With too much depth the stress can exceed the elasticity of the paper causing fibers to rupture and the paper to crack.
- The press: The etching press provides the high pressure needed for most embossing, but some artists use hydraulic presses for very deep relief. Too much pressure can cause cracking due to excess stress on the paper.
- The paper: Long-fibered papers are better able to undergo the plastic elongation needed to conform to the shape of the plate and retain embossing without bursting. Since the paper is dampened before embossing to take advantage of the increased plasticity and flexibility of the swollen cellulose fibers, the moisture sensitivity of the paper is important. Heavy papers generally produce better quality embossing and retain it better on drying. Handmade rag papers are better than machine made papers which have a stronger directional response to water.
- With any treatment care must be taken not to damage or reduce the relief. Drying and flattening without flattening the embossing is problematic for printmakers, as well as conservators who have to consider this before undertaking any aqueous treatment. The dimensional stability of the paper may be a deciding factor in whether or not to treat the object. Sometimes embossed and unembossed areas of the same sheet will have very different dimensional responses to moisture. Some embossed prints require a great amount of moisture to relax and flatten all areas. Soft felts or blotters can be layered and “sculpted” to protect relief areas as the print is dried under pressure. A heavy embossed paper may be able to withstand, and may even require, a surprising amount of weight to flatten it. Conversely, to retain more delicate embossings it may be necessary to limit the use of flattening techniques until the work is almost dry. Stretch drying is a possibility but may reduce the embossing as the paper contracts. Another possibility is drying on the suction table, with relief areas masked out, if necessary, to prevent their contraction under vacuum pressure.
- Repairs to embossed areas must be made with papers that are flexible enough to conform to the embossing. Mends can be held in place by finger pressure, while drying with wads of cotton covered with a non-woven polyester, or other malleable, absorbent materials.
- Mounting, matting and framing must provide adequate support and depth.
- Damage to structural components (e.g., plaster) and secondary mounting materials as well as the wallpaper itself; media friability.
- The type of damage will dictate if the wallpaper can be treated in situ or if removal is required. Treatments include plaster repairs, readhering cleavage between mounting layers, media consolidation, compensation, and rehanging/protection.
The composite nature of globes, the hidden intricacies of their internal structures, their sizes if large, and their shape present unique problems. In addition, it was common practice to update and recover the gores because of their utilitarian function.
- Mechanical damage: The surface of the globe gores becomes abraded if the sphere is inaccurately mounted in its stand or if the globe drops in its horizon ring. The internal wooden structure, papier-m&acaron;ché and plaster components may warp and move, resulting in plaster cracks. Fractures radiate out from holes in the sphere, with associated losses of ground, paper, and design. It is not uncommon for the bag of lead shot inside the globe to burst. The paper surface on the horizon circle may also suffer from losses, discoloration and soiling.
- Discoloration of the varnish layer: Dust settles directly on the Northern area of the globe. Therefore, the Southern Hemisphere is usually cleaner and has a tougher coat of varnish. The varnish layer and surface dirt may obscure information recorded on the globe gores.
- Insect, microbial damage: The wood, paper, glue, and paste used to construct globes can become infested, including the inner wooden structure and the wooden stand resulting in losses of component materials and weakening of the globe's structure.
- Examination: The construction and condition of both the external and internal components of the globe must be determined using established non-destructive methods. Directing an x-ray beam at different points of the sphere will provide information about the internal structure of the globe. Examination under ultra-violet fluorescent illumination will help identify the varnish layer, retouches, and patches. An infra-red vidicon imaging system can intensify surface information on the sphere that is hidden by a discolored varnish layer and surface soiling. Details about the maker, the construction location, and the date should be recorded. This information may be contained in the cartouche or nameplate on the sphere. The stand and any metal components should also be examined and described in the examination record. Refer to Baynes-Cope 1985; Lewis, Leanne, and Sumira 1988; Sumira 1989; and van der Reyden 1988.
- Surface cleaning: It is essential to remove the globe from its horizon circle and meridian ring before cleaning. Brush the surface of the sphere with a soft brush followed by dry cleaning, wiping with a slightly dampened swab, or the application of a thick poultice of methyl cellulose. The materials used to color the globe gores and horizon circle, usually watercolors, may be extremely fugitive. Solvents, such as dilute ammonium hydroxide may help remove surface dirt and speed drying time. Dismantling and immersion of the globe gores in water is a drastic measure. Upon drying, the paper gores may shrink, thereby distorting the intended geographical distance. Repositioning the gores on the sphere requires great skill as they must be adhered accurately with a very slippery paste while they are saturated with moisture.
- Varnish removal: It is preferable to remove varnish mechanically. If deteriorated and originally applied over size layer, the varnish will flake off cleanly when abraded with a scalpel edge or point. The varnish layer may sometimes be removed mechanically using a tool (e.g., a rounded orange stick – a manicurist's tool). This avoids the use of chemicals and can result in dramatic cleaning.(LP) Rapid acting solvents on a small swab of cotton wool should be used if a decision is made to remove the vanish layer in this way. The use of chemicals should be limited since rinsing opportunities are restricted while the gores are adhered to the sphere. It may not be possible to remove the varnish layer if the globe was varnished without sizing the paper support. Solvents may drive the surface dirt into the paper, staining the globe gores.
- Reducing dents: It may be possible to apply moisture from within the sphere if a hole has occurred in the area of the dent. Unobtrusive dents may be left as is. Bridges constructed of aluminum mesh or fiberglass will support damaged areas on the inner papier-m&acaron;ché shell.
- Repair of damaged plaster: The damaged area should be allowed to dry out before starting to in-fill. Apply the filling material in several applications to speed the drying time. A base coat of dental plaster “Kaffir D” (10:1 with water) will minimize the amount of shrinkage (Leyshon 1988). An example of a plaster mix for filling damaged areas (resembling original composition of the plaster used for the Senex globes): 1 part rabbit skin glue gelatin; 9 parts kaolin (B.P.); 1 part finely precipitated chalk (pure calcium carbonate – can be varied with gypsum or French chalk). The mixture was applied hot and allowed to dry between each application. Sizing the final coat of plaster reduces its absorbency.
- Repairs to internal structure (e.g., retrieving the lead shot bag and reconstructing the North and South Poles). See Baynes-Cope 1985.
- Repair of damaged paper support: Repair missing areas with chamfered infills of paper similar to the original in thickness, density, color, translucency, chain and laid lines, and surface texture. More than one thickness of paper may be required for fills on different areas of the sphere. Old plaster is extremely porous. Applying an impervious layer to the plaster base may be required before the fill is adhered. Blot the repair with a soft absorbent blotting paper to reduce drying time.
- Revarnishing: If a decision is made to revarnish the globe following treatment, tests must be conducted to identify a varnish which will be deposited only on the surface of the globe gores, thereby retaining reversibility and the refractive index of the paper (van der Reyden, 1988). The porosity of the paper must also be determined. Resizing of the gores is often necessary.
- Display: A hemispheric dome structured out of ultraviolet filtering Plexiglas will help protect the globe. The dome can be fitted to the horizon ring (Leyshon 1988).
- The quality of the board and paper used to construct these boxes is generally acidic and deteriorates over time under adverse environmental conditions. The boards themselves can warp and sag. Adhesives at the joins weaken and fail, and the boards become detached or are lost. If the boards were stitched together the threads can loosen and break. The papers on the interior and exterior can delaminate, crack along seams, and become abraded and stubbed from general use. Poor storage conditions also present the problems of surface dirt, insect accretions and water damage.
- The artifacts in the box itself can also contribute to its overall condition. Boxes which have held heavy items suffer from loose or completely detached bottom boards. The action of removing and returning an item to its box can cause abrasions to both artifacts.
- Conservation treatment: Boxes offer a unique challenge to paper conservators. Traditional methods of repair need to be modified to conform to the three dimensional shapes of these objects. Bulldog clips, clothespins, and small clamps can be used to hold tears and splits in place after mending. Smaller boxes can be wrapped with Teflon tape or Ace bandages to secure a mend or adhesive in place. Often with small boxes, a secondary support needs to be constructed and placed inside the box in order to provide additional support prior to wrapping. Losses can be inserted with a board similar in thickness to the original and covered with toned Japanese or Western paper as necessary. Mends or reinforcement may need to be placed on the interior and exterior in order to provide additional overall support to the box. Water damage may require inpainting since aqueous treatment can be difficult to carry out due to paper layers and the shape of the item.
- Storage and display: Empty artifact boxes should be displayed and stored with an interior support which helps to maintain the box's shape and prevents the lid from sagging. This can be constructed from thin, acid-free board as a series of vertical, accordion folded strips or as a scored, folded, and taped open ended form. Boxes which hold artifacts can be stored on a secondary support of acid-free corrugated cardboard slightly larger than the dimensions of the box to allow for a hand hold. The box itself can be held in place by attaching twill tape to the underside of the secondary board and tying the tape over the box. Artifact boxes can also be placed within a custom-made or commercially made storage box.
Other Objects Made By Distortion of Planar Sheet
Scoring, folding, rolling, and curling are the basic methods by which the flat plane of a sheet of paper can be shaped into a three-dimensional form. Adhesives or fasteners may be used to keep the sheet in the distorted form.
- Deterioration of the object with aging is affected by environmental factors and all the inherent vices of its materials and construction, but can be especially devastating because the breakdown of the paper (or adhesive) can lead to the collapse of the three-dimensional structure. The three-dimensional construction may preclude, or at least complicate, more interventative treatments like washing and lining. Techniques may be borrowed from treatments used in textile conservation, such as the use of minisuction tables with shaped heads that can be inserted where needed for local washing or solvent treatment.
- Display and storage: Among the standard considerations for works of art on paper, relative humidity deserves special attention. Embrittlement caused by low humidity may result in breaking at the folds or the areas which most support the weight of the object, while the increased flexibility that occurs in high humidity may result in sagging and sometimes collapse of the object. Even in the best of conditions structural support is often required, both in storage and display.
Traditional Non-Paper Supports
- Uncertainty about the manufacturing process presents problems: if starch paste was used in bonding then aqueous treatments could endanger the adhesion of the two layers forming the sheet.
- Analysis has shown that proportions of the main constituents of papyrus (cellulose and lignin) vary with age, manufacturing process, and environmental effects. If well-made, properly housed, and cared for, papyrus can be a durable material which may be repeatedly rolled and unrolled over time. Eventually its flexibility diminishes; ancient papyrus may now be desiccated and brittle as well as discolored. It also has a strong tendency to curl up unless restrained. Edges fray easily. Nineteenth and twentieth century methods of handling, storage, and display often consisted of taping or gluing the papyrus to cloth, poor-quality cardboard, cellulose nitrate, hardened gelatin sheets, or clamping between sheets of glass in passe-partout. Acids have migrated from these materials into the papyrus. In addition, papyri within such mounts have fractured because of tensions between object and support in fluctuating atmospheric conditions (Elliott 1987, 64).
- Alignment of fragments: Pronounced fibers of cross-laminate structure, obvious on a light table, may assist in positioning improperly placed fragments. Deteriorated papyrus may be so brittle that it is impossible to handle without dampening; however, its surface becomes tacky when wet. Nylon gossamer tissue is used as a work surface at the British Museum. Overall moistening is recommended to prevent formation of stains that occurs with local wetting; a solution of 1:1 industrial methylated spirits (IMS), (or ethanol or acetone), and water permits alignment of fibers, manipulation of distortions, removal of creases, etc.
- Backing removal: Removal of fragile, brittle papyrus from poor quality secondary support is assisted by using a facing. Some poultices (cellulose ether, sodium carboxy methyl cellulose [SCMC]), damp blotter method or both have been used to remove backings, inlays, and old repairs. Scrape away residues in the direction of the papyrus fibers to avoid damage.
- Aqueous treatments: Discolored and stained papyrus apparently responds well with no layer separation problems. In order to remove discoloration and acidity by washing, the sheets must be reasonably sound. Float washing on Mylar or between two sheets of nylon gossamer web is recommended; papyrus' natural buoyancy contraindicates immersion.
- Repair: Papyrus has a strong tendency to return to the position it has been held in over a long period of time (e.g., rolled). At the British Museum, gluten-free wheat starch and Japanese paper were used to repair papyrus successfully on the light table.
- Some papyrologists feel that repairs on literary texts and archival documents should be visible so that the origin of the texts' arrangement is clear. This will aid interpretation of the text. Before treatment photography is, of course, also helpful.(KDB)
- Removal of acidity: pH of papyrus is acidic because of its relatively high lignin content (unless formerly buried in alkaline conditions).
- At the Princeton Library, a papyrus mask from a mummy (dating from Ptolemaic times) was disassembled in order to ascertain presence of informative texts or documents. A Danish freeze/dry technique was used in which the object was soaked in an enzyme (to dissolve the adhesive) and then freeze-dried to remove the water and adhesive. In addition, some parts required steaming in order to release them.(KDB)
- Palm leaf is very susceptible to desiccation by a hot, dry environment; it will lose flexibility and become brittle. The lignified cells are particularly susceptible to degradation and discoloration.
- When exposed to high RH conditions or actual wetting the leaves may stick together in solid blocks.
- Palm leaf has poor resistance to wear and tear; it is easily damaged by constant handling, especially at the edges which can fray.
- The leaf tends to split into long strips along the longitudinal veins, especially where incised previously with a stylus. Once begun, mechanical damage progresses through the leaf.
- Damage is caused by friction between the cord and the edge of the hole.
- Correct storage in a controlled environment is the best way to prevent damage to palm leaf manuscripts and should be designed to minimize the need for unnecessary handling. (See Lawson 1983 for current practices at the British Library.) To lessen effects of damage from lacing, the British Library strings the leaves into books using the left hole only.
- Palm leaf manuscripts with very small holes, there by tradition rather than for practical use, should not be strung.
- Parchment is a relatively stable material in that it is resistant to deterioration. It absorbs few sulfurous acidic pollutants and those it does tend to be absorbed by its natural alkalinity.
- Parchment is very hygroscopic; a humid environment makes it swell, a dry atmosphere dehydrates it so that it shrinks and becomes stiff. It is the ground substance which is extremely reactive to humidity and can absorb water even after dried in the parchment. If parchment absorbs large amounts of water, the fiber network can relax since it is not constrained. When the fiber network system is dried in this new relaxed state, the parchment can become hard, horny, and cockled. Therefore, exercise extreme caution when storing or treating parchment. To retain the properties of parchment, any treatment involving humidity should also involve drying under tension to maintain the stressed, parallel alignment of fibers.
- Dimensional changes in the parchment support caused by relative humidity fluctuations can create tensions in the parchment which can cause detachment of media.
- High humidity levels will lead to microbial attack on parchment and consequent weakening and staining. It also enhances the usual chemical degradation reactions (e.g., excessively acid inks can transform the support into lacework) (Chahine 1989, 15).
- Can be easily torn or cracked if the skin has suffered from deterioration, is thin, and/or the conditions are too dry with excessive stress.
- Greek medieval (Byzantine) artists coated the finished parchment sheet with an egg-white preparation and polished it; this created a smooth, shiny surface from which media readily flakes (Abt and Fusco 1989, 61).
- Often the same color as paper, very thin and flexible, though with a “solid” feel and a tough “body,” parchment can easily be mistaken for a sturdy paper. Parchment's behavior and recommended care, however, are radically different from that of paper, because of the great differences in basic natural materials from which each is made. When parchment is mistaken for paper and subjected to certain paper conservation procedures, the results are disastrous (Ellis 1987). Parchment cannot be immersed in water, for instance, because the lime can be removed, and the skin can wrinkle and go transparent. Exposure to heat is disastrous as the skin can irreversibly shrink.
- Since parchment is so hygroscopic, one can expect it to expand and contract with seasonal changes in RH and temperature. A certain amount of cockling in an item considered for treatment is not only inevitable but also aesthetically inherent. Concern must be given to cockles affecting media attachment. Traditional methods of hinging using paste and Japanese tissue can result in cockling around the hinge as the skin expands and contracts, while the pasted hinge area moves at a different rate. Hinging methods have included string matting (see Clarkson 1987, 201–209), suspending with Mylar tabs and applying the feathered fiber ends of Japanese paper strips all around the perimeter.
The methods used to treat parchment are based on those used to originally prepare it.
- Surface cleaning: Use brushes, soft erasers, low suction vacuum, swabs, and a minimum amount of moisture. One must be very careful that eraser particles do not become trapped in the fibrous surface of the parchment, especially in areas where the surface is creased or abraded.
- "Performing miracles on water-staining and grime can't really be expected since the skin cannot be immersed in water" (Munn 1989, 30). Use the least moisture possible to remove water-soluble adhesive residues. Try ethanol and water mixtures and work locally under the microscope. Use of the suction table may be effective for local stain removal as well as flattening.
- Appearance of transparency in the course of conservation treatments, especially as a result of the application of water, water/alcohol, and urea solutions, lanolin, glycerol, excessive tension, etc. (Chahine 1989, 17–18).
- Methods of repair should "aim to preserve the original character of the material by using methods related to the parchment-making process, in particular...hydration and tensioning" (Cains 1982/83, 15).
- Water-damaged or distorted parchment may respond to humidification in a constant humidity chamber, on a damp pack of blotters through several layers of permeable polyester web or Gore-Tex, or overall applications of alcohol or alcohol/water solutions. "The advantage of the chamber method is that the hydration process is slow and one can determine the best conditioning point within a broad time scale"; timing with the pack system, particularly if the parchment is thin or there is a danger of offsetting, can be critical (Cains 1982/83, 16; Munn 1989, 31). With the pack there is a risk of transparency and/or excess water absorption.
- Extra humidity may be applied to more severely affected, horny, or less absorbent local areas during overall humidification; use moist, not wet, blotter pieces over permeable polyester web on distorted areas or apply water/alcohol solutions locally. Water alone can darken parchment.
- The appearance, opacity and surface texture of parchment can be altered during hydration and tensioning (Cains 1982/83, 15–16).
- Flattening/Tensioning: Pressure methods of flattening do not preserve the original character of parchment nearly as well as tensioning which reflects the original parchment-making process (Cains 1982/83, 15). Tensioning "must restrain the skin while it is drying until the moment of reaching equilibrium when the skin comes under tension and is more or less flat." The relaxed condition of the humidified skin may lead to overstretching; with very distorted parchment, tensioning may be undertaken gradually in a series of steps (Cains 1982/83, 15–17). If dried too fast after humidification distortion may result.
- Poorly modified clips combined with high moisture content in the skin will produce indelible marks around its edges.
- Applications of lubricants to shrunken material that does not respond to hydration and flattening (see Chahine 1989, 17–18).
- When mending skin use only structurally similar materials (e.g., gelatin or parchment size for the adhesive, parchment and goldbeater's skin or fish skin membrane for the mending materials). This should prevent stresses resulting from different expansion/contraction rates which may cockle and tear the parchment.
- Because of its extreme hygroscopicity it is essential to keep parchment in a stable environment: 18°C ±2° (64.4°F ±2°), 55% RH ±5% (Chahine 1989, 15). The benefits of flattening parchment can be largely negated by dry storage or exhibition. Maintain a micro-climate within exhibition cases that will conserve the equilibrium moisture content of the parchment, see, for example, Cains 1982/83, 21.
- Media consolidation is frequently necessary. Use parchment size in various dilutions with water and ethanol or isopropanol. Apply locally with brush or spray when there is overall media friability. Press after spraying if possible.(LP)
- Pith "paper" is so fragile that pressure from a finger can create a permanent depression (seen frequently on these objects) and a finger nail easily slices it. Use a secondary support whenever possible to avoid direct contact. The porosity leads to easy discoloration by embedded dust, severe staining – even from materials applied to the back (e.g., original mounting adhesives). The appearance of the pith is such that tissue fills are very obvious. If scraps of pith are available for filling, be sure to match grain directions. Scraps of a different tone can be lightly brushed with dry pigment mixtures to improve color compatibility. Splits have often drawn apart, with resultant gaps.(CS)
- Pith "paper" is quite flexible in humid air and can be stretched and molded when damp. Water and some organic solvents may make it temporarily transparent. Wetting or washing by immersion will expand the support permanently. It becomes more brittle with drying and even when new it has poor fold resistance. It may curl or crack with exposure to excessive heat. The fragile surface is easily damaged by abrasion and by uneven or excessive pressure. Pith "paper" becomes brittle with age, it cracks and tears easily when improperly handled or stored.
- Presentation: Traditional presentation was by ribbon binding around all edges (most likely to protect against splitting) and then assembly of individual sheets into a bound volume (Purdue and Kraebel 1961, 177). In its original form, it is likely to be found mounted on album pages of good quality paper (Chinese/European). Poor-quality European secondary supports are likely to be of later origin. Often paintings are only tipped on or otherwise locally attached. Rapid expansion and contraction of sheets with humidity changes can lead to physical damage if they are restricted by glued areas and mounting methods.
(See also Rickmann 1988.)
- The pith sheet's surface is very delicate and porous. Avoid removing surface deposits by brushing, this may embed mold or dirt. Do not use a scalpel to pop off accretions, this will only cause more problems.(CS)
- It is very difficult to mend tears because of both translucency of the material and difficulty in manipulating it. F. Mowery's gossamer tissue (or as a second choice tengujo) impregnated with Klucel G and applied by rolling a dryish swab of ethanol over the tissue works well. To set: immediately place Teflon cloth over the swabbed tissue, press lightly with fingers and blow away the ethanol.(CS)
- Pith sometimes shows foxing or glue staining. Stains can be successfully treated locally with water and blotting paper. Use of the vacuum suction table may not be safe because pith is so spongy, but with some sheets it can be used at very low suction.(CS) To a certain extent, strength and flexibility of pith “paper” is enhanced with wetting so aqueous methods of repair would seem to be the methods of choice. Yet, most conservators use only a minimum amount of moisture. This is because the pith paper tends to absorb water like a sponge; on these vividly painted objects at least one pigment always seems to be extremely prone to wicking upon exposure to water (as opposed to moisture vapor).(CS) Some conservators use methyl cellulose as adhesive to control water content during lining and mending.
- Pith paper should not be lined unless it is very fragmented since puckering (and slight relief effect) of the support caused by the pigment layers is original. Since tears/splits have no overlap, and thus are difficult to repair successfully, lining is sometimes necessary. To avoid pressure on surface when a pith “paper” support must be lined and flattened, and to eliminate severe curl and tenting at cracks after lining, a modified “polyester lining” technique may be used. Sanded Mylar is taped to solid, flat surface. Woven polyester fabric is laid on Mylar, impregnated with very thin paste and stretched out evenly. Japanese paper is brushed out on fabric and allowed to dry. Lining paper is coated with thin layer of relatively viscous methyl cellulose, humidified pith “paper” is set on lining, gently aligned and allowed to dry. Then Mylar and polyester are each peeled off back without need to strain and crack pith “paper.” More traditional methods using Japanese papers and wheat starch paste can also be successful. Make lining and presentation system sufficiently larger around edges to minimize exposure to handling.(CS) Minimum pressure must be used at all times or the pith surface becomes “dead” or flat. On the other hand, previous mounting or storage may leave the sheet quite compacted before it arrives for treatment. In such cases, controlling other factors may become more important.(CS)
- When missing areas must be replaced only butt joins are suitable; match the grain directions. Apparently, pith paintings can still be bought in Hong Kong, which could be an option for obtaining repair material.
- Display: Pictures that have been cut from their albums in the past should be individually displayed. It is possible to “cradle” each sheet so that there is no application of paste to the pith, nor any restriction of movement by hinges. Cut strips of a suitable material and paste along outer edges to mat backing board so that inner edges of strips overlap pith sheet and hold it securely in place. An eight-ply overlay window mat will ensure adequate protection for the fragile pith surface. This method is not suitable for album display.
- Light-sensitive colorants: In particular, modern tapas may feature inks from felt-tipped pens.
- Water-sensitive colorants, especially "smoked" tapa; water-sensitive adhesive joins between the individual tapa pieces forming the composite object. Joins may separate when wet.
- Glossy surface coating of coconut oil is susceptible to mold (Green 1987, 59).
- Storage and display problems for very large pieces. Traditional folding for storage causes deformation and breaking of fibers.
- Delamination of layers (with age, washing) and usual problems (cracks, holes, tears).
- Frequently acidic and brittle.
- Soiling from wear and greasy, sooty dirt accumulated from cooking fires can be a clue of dating (Green 1986, 20).
- Some may retain rolled or distorted shape of the tree.
- See Green (1986, 20) for factors to consider; in surface cleaning and washing must not remove ethnographic evidence (soils) for history and use.
- Cleaning: Vacuuming is acceptable for removal of dust. Take care with paints as they can be friable depending upon binder.
- Crease removal: Wetting, steaming, and humidification have all been tried with limited success. Tapa must be handled with great care and adequate support when wet because its strength may decrease.
- Tear repair: Mulberry paper is satisfactory for tears and small voids.
- Backing/Lining is a treatment of last resort for tapas which are structurally insecure and which would not be adequately supported with patch-type repairs. Linings may obscure previous repairs which may be historically significant. Embossing, if present, should remain visible. In addition, embossing may make it difficult to adhere the backing. Linings also contribute to a loss of flexibility. Lining materials include Japanese paper and contemporary tapa (the latter is preferred, in part because it conforms more readily to the surface irregularities of the tapa primary support). Starch paste or cellulose-derived adhesives are preferred, particulary the latter because in any future analysis it will not be confused with the original adhesive. Nylon laminating tissue and stitching have also been used to adhere linings.
- Filling voids: See tear repair, above, for treatment of small voids. Larger voids need backing or pulp fills. The latter is the standard treatment and uses coarsely processed pulp.
- Mounting methods include hinge mounting, pressure-mounting, clips, etc.
Drafting Cloth ("linen")
- The textile substrate is very durable and will withstand much abuse. However, a starch or gelatin filler/coating can be destroyed by moisture resulting in distortion, opacity, exposed fibers, and limpness.
- The starch or gelatin coating renders drafting cloth susceptible to damage from mold, insects, vermin and foxing.
- Heavily filled/coated: Ink and watercolor will not penetrate drafting cloth and, therefore, their application is not permanent. May be washed off with moisture or smeared if handled poorly.
- Storage and handling: Rolling, folding, and poor handling techniques crack the coating and will cause it to wear off gradually. Eventually, the cloth will fray around its outer edges.
- Mold removal may be successfully accomplished using a vacuum aspirator.
- Dry cleaning to remove superficial grime is safe only when the surface is in excellent condition (a smooth, unfractured coating). Eraser particles can become embedded in exposed fibers or “rub out” the fragile coating. Swabbing with ethanol often releases surface grime.(LP)
- Selected organic solvents have been used with success to reduce staining, adhesive residues, etc. Some linens benefit from cleaning with water and ethanol mixtures.(LP)
- Mend with heat-set tissue or aqueous adhesives, however, drafting cloth may be heat-sensitive, especially when degraded. Aqueous adhesives will disturb the starch or gelatin filler/coating. Coating can be approximated by applying methyl cellulose and burnishing through polyester film.(LP)
Contemporary Non-Paper Drawing Supports
Polyester Drafting Films
- It is difficult to start a tear in polyester drafting films but, once started, the tear extends easily.
- Conventional mending and hinging adhesives for paper are incompatible with drafting films. Synthetic adhesives, whether solvent or heat activated, must be tested for compatibility with each film, since some films are heat or solvent sensitive.
- Synthetic hinging materials (Hollytex, Cerex, etc.) have been used with success. These materials, once impregnated with a synthetic adhesive (Lascaux 498–20x, etc.) can be heat or solvent activated. The translucent appearance of the hinges renders them almost invisible. (AM) Double-sided tape has also been used for hinging plastics. (KDB)
- Large and oversized pieces may have been folded. Humidification is not generally effective. Flattening may be achieved by light application of heat and pressure (conventional tacking iron and silicon release paper) on crest of crease. (SP)
- Reformatting (e.g., microfilming) should be considered for architectural drawings on unstable plastic although this option is not applicable to fine arts pieces. (LP)
- AIC-BPG. Paper Conservation Catalog - 19, Bleaching. Washington, DC: AIC-BPG, 1989.
- AIC-BPG. Paper Conservation Catalog - 24, Backing Removal. Washington, DC: AIC-BPG, 1985.
- AIC-BPG. Paper Conservation Catalog - 29, Lining: 40. Matting and Framing. Washington, DC: AIC-BPG, 1988.
- Balston, Thomas. James Watman: Father & Son. London: Methuen & Co., Ltd., 1957.
- Bachmann, K. “The Treatment of Transparent Papers: A Review.” The Book and Paper Group Annual 2, 1983, pp. 3–14. Extensive earlier bibliography.
- Banks, Paul. “Environmental Conditions for the Storage of Paper-Based Records.” Proceedings of Conservation in Archives: International Symposium, Ottawa, Canada 1988. Paris: International Council on Archives, 1989, pp. 77–88.
- Boston Museum of Fine Arts. Rembrandt: Experimental Etcher. Boston: Boston Museum of Fine Arts, 1969.
- Britt, Kenneth W., ed. Handbook of Pulp and Paper Technology. 2nd edition. New York: Van Nostrand Reinhold Co., 1980.
- Browning, B.L. Analysis of Paper. 2nd edition, revised and expanded. New York: Marcel Dekker, Inc., 1977.
- Byers, W. “Cracking at the Fold Problems.” Graphic Arts Monthly 43, No. 5, May 1971, pp. 104–110.
- Casey, James P., ed. Pulp and Paper: Chemistry and Chemical Technology. 3rd ed. New York: John Wiley and Sons, 1981, Vol. 3 “Loading and Filling,” pp. 1515–1546.
- Clapperton, R.H. and William Henderson. Modern Papermaking. London: The Waverly Book Co. Ltd., 1929.
- Cohn, Marjorie B. “A Hazard of Float Washing: Regeneration of Paper Sizing.” Book and Paper Group Postprints. Washington, DC: AIC, 1982, 13 pages plus 2 tables.
- Collings, Thomas and Derek Milner “The Nature and Identification of Cotton Paper-Making Fibers in Paper.” The Paper Conservator 8, 1984, pp. 59–71.
- Collings, Thomas and Derek Milner. “The Identification of Non-Wood Paper Making Fibers: Part 3.” The Paper Conservator 7, 1982/83, pp. 24–27. (Esparto and Manila Hemp.)
- Cook, J.G. “Ramie.” Handbook of Textile Fibers Vol. 1 - Natural Fibers. Merrow: Durham, 1984, pp. 22–24.
- Cumberbirch, R. “Why A Fiber Works.” The Shirley Link, 1974, pp. 147.
- Daniels, Vincent. “The Discoloration of Paper on Aging.” The Paper Conservator, 12, 1988, pp. 93–100.
- Daniels, Vincent and Lore E. Fleming. “Cockling of Paper in Museums.” Symposium 88: The Conservation of Historic and Artistic Works on Paper. Ottawa: Canadian Conservation Institute. (In press - Fall 1990.)
- Dwan, Antoinette. “Examination and Conservation of Nineteenth Century Japanese Papers.” Typescript of a paper presented to the Book and Paper Group of the American Institute for Conservation 17th Annual Meeting, Cincinnati, 1989, 18 pp.
- Ellis, Margaret Holben. “A Practical Approach to Drawings Storage.” Drawing 1, No. 6, 1980, pp. 132–134.
- Ellis, Margaret Holben. The Care of Prints and Drawings. Nashville, TN: AASLH Press, 1987.
- Feller, R. “The Deteriorating Effect of Light on Museum Objects.” Museum News 43, Technical Supply No. 3, 1964, pp. i–viii.
- Hills, Richard L. Papermaking in Britain 1488–1988: A Short History. London: The Athlone Press, 1988.
- Hunter, Dard. Papermaking: The History and Technique of an Ancient Craft. New York: Dover Publications, Inc., 1978.
- Keyes, K.M. “The Unique Qualities of Paper as an Artifact in Conservation Treatment.” The Paper Conservator 3, 1987, pp. 4–8.
- Krill, John. English Artists Paper. London: Trefoil Publications Ltd., 1987.
- Labarre, E.J. A Dictionary of Paper and Paper-Making Terms. Amsterdam: Swets and Zeitlinger, 1937.
- Long, Paulette, ed. Paper - Art and Technology. San Francisco: World Print Council, 1979.
- McAusland, Jane and Phillip Stevens. “Techniques of Lining for the Support of Fragile Works of Art on Paper.” The Paper Conservator 4, 1979, 33–44.
- Meder, Joseph. The Mastery of Drawing. Translated and revised by Winslow Ames. New York: Abaris Books, Inc., 1978.
- Miles, Catherine E. “Wood Coatings for Display and Storage Cases.” Studies in Conservation 31, 1986, pp. 114–124.
- Padfield, Tim, David Erhardt and Walter Hopwood. “Trouble in Store.” Science and Technology in The Service of Conservation, Preprints of the ICC Washington Congress. London: IIC, 1982, pp. 24–27.
- Priest, D.J. “Modern Paper.” Modern Art: The Restoration and Techniques of Modern Paper and Prints. London: UKIC, 1989, pp. 5–7.
- Roberts, Matt T. and Don Etherington. Bookbinding and the Conservation of Books; A Dictionary of Descriptive Terminology. Washington, DC: Library of Congress, 1982.
- Shahani, C.J. and F.H. Hengemihle. “The Influence of Copper and Iron on the Permanence of Paper.” Historic Textile and Paper Materials: Conservation and Characterization. Washington, DC: American Chemical Society, 1986, pp. 386–410.
- van der Reyden, Dianne. “Technology and Treatment of a Folding Screen Comparison of Oriental and Western Techniques.” The Conservation of Far Eastern Art: Preprints of Contributions to the Kvoto Congress. London: IIC, 1988, pp. 64–68.
- Weidner, Marilyn. “Damage and Deterioration of Art on Paper Due to Ignorance and the Use of Faulty Materials.” Studies in Conservation 12, No. 1, 1967, pp. 5–24.
- Watrous, J. The Craft of Old Master Drawings. Madison: University of Wisconsin Press, 1957.
- Wehlte, Kurt. The Materials and Techniques of Painting. New York: Van Nostrand Reinhold, 1982.
Mechanical Wood Pulp Papers
(See also General References)
- Hon, David N.S. “Discoloration and Deterioration of Modern Papers.” Science and Technology in the Service of Conservation, Preprints of Contributions to the IIC-Washington Congress. London: IIC, 1982.
- Lyall, Jan. “A Preliminary Study of Chemical Methods for Stabilizing Lignin in Groundwood Paper.” Science and Technology in the Service of Conservation, Preprints of Contributions to the IIC-Washington Congress. London: IIC, 1982, pp. 79–84.
- Shahani, D.J. “Options in Polyester Encapsulation.” Association of Canadian Archivist Bulletin 2, No. 1, 1986, 1 page.
- Young, G.S. and Helen Burgess. “Lignin in a Paperboard Advertised as Lignin-free.” IIC-CG Bulletin 14, No. 4, 1989, pp. 14–16.
(See also General References)
- Perkinson, Roy. “Observations in the Drawings of Winslow Homer.” The Book and Paper Group Annual 5, 1986, pp. 1–8.
- Samuels, Laurie. “Optical Brighteners in Paper.” Papers Presented at the 15th Annual Art Conservation Training Programs Conference. Harvard University Art Museums, 1989, in press.
- van der Reyden, Dianne and Nancy McRaney. Identification of Colorants for Paper. Smithsonian Institution, Conservation Analytical Laboratory: Washington, D.C., 1990, unpublished.
(See also General References)
- Daniels, Vincent. “A Study of the Crystallinity of Paper Before and After Conservation.” The Paper Conservator 10, 1986, pp. 70–72.
Artists' Coated (Prepared)
(See also General References)
- Cennini, C. The Craftsman's Handbook. Translated by D. Thompson, Jr. New York: Dover Publications, Inc., 1954, pp. 6–7.
- DaVinci, Leonardo. Treatise on Painting. Translated by P. McMahon. Princeton: Princeton University Press, 1956, p. 105.
- Ellis, Margaret Holben. “Metalpoint Drawings: Special Problems for Collectors.” Drawing 2, No. 3, 1980, pp. 59–61.
- Richmond, Alison, “Turner's Use of Paper up to 1820' - A talk given by Peter Bowers.” Paper Conservation News, No. 54, 1990, p. 4.
(See also General References)
- Baker, M., D. van der Reyden, and N. Ravenal. “FTIR Analysis of Coated Papers.” The Book and Paper Group Annual 8, Washington, DC: AIC, 1989, pp. 1–12.
- Casey, James P., ed. “Pigment Coating.” Pulp and Paper: Chemistry and Chemical Technology. New York: John Wiley and Sons, Vol. 4., 1983 “Pigment Coating,” pp. 2018–2189.
- Parker, A.E. “The Freeze-Drying Process: Some Conclusions.” Library Conservation News, No. 23, 1989, pp. 4–6, 8.
- Prosser, Ruth. “Pigment Coated Printing Papers.” Modern Art: The Restoration and Techniques of Modern Paper and Prints. London: UKIC, 1989, pp. 8–12.
- Lattuati-Derieux, A., Egasse, C., Regert, M., Chung, Y., Lavédrine, B., 2009. “Characterization and degradation pathways of ancient Korean waxed papers”, Journal of Cultural Heritage, Vol 10, pp. 422–427.
- A collection of Korean waxed papers from the 15th-16th centuries were chosen to be studied because they were starting to present signs of deterioration. These included: traces of mould, folds, cracks, embrittlement of the wax and white or purple deposits on the surface. The authors of this paper used Fourier Transform Infrared (FT-IR) spectra and gas chromatographic and mass spectrometry investigations to identify the biomarkers and degradation markers of the Korean paper samples. Four different samples of waxed paper were taken. Comparing the samples to a modern sample of Korean beeswax showed that the chemical composition was very similar to the ancient Korean beeswax samples found on the papers. The main degradation compounds were found to be hydroxyethers.
(See also General References)
- Anderson, Priscilla. “Transparent Paper: An Examination of its Uses Through Two Centuries.” Senior essay, History of Art Department, Yale University, New Haven, Connecticut, 1990.
- Bachmann, K. “Transparent Papers Before 1850: History and Conservation Problems.” New Directions in Paper Conservation. The Institute of Paper Conservation 10th Anniversary Conference, Conference Notes. Oxford, England: Institute of Paper Conservation, 1986, p. D61 (abstract).
- Flamm, Verena, Christa Hofmann, Sebastian Dobrusskin, and Gerhard Banik. “Conservation of Tracing Papers.” 9th Triennial Meeting of the ICOM Committee for Conservation Preprints. Dresden, German Democratic Republic: ICOM, in press 1990.
- Fletcher, Shelly and Judy Walsh. “The Treatment of Three Prints by Whistler on Fine Japanese Tissue.” Journal of the American Institute for Conservation, 18, No. 2, 1979, 118–126.
- Futernick, Robert. “Methods and Makeshift: Stretch Drying Lined Artifacts.” The Book and Paper Group Annual 3, Washington DC: AIC, 1984, pp. 68–70.
- Keyes, Keiko M. “The Use of Friction Mounting as an Aid to Pressing Works on Paper.” The Book and Paper Group Annual 3. Washington DC: AIC, 1984, pp. 101–104.
- Mills, John S. “Analysis of Some 19th Century Tracing Paper Impregnates and 18th Century Globe Varnishes.” New Directions in Paper Conservation. Oxford, England: Institute of Paper Conservation, 1986.
- Priest, Derek. “Paper Conservation Science at UMIST.” The Paper Conservator 11, 1987, pp. 73–80.
- Rundle, C. “The Composition and Manufacture of Modern Tracing Papers.” New Directions in Paper Conservation. Oxford, England; Institute of Paper Conservation, 1986, D64–65 (abstract).
- Wilson, Helen. “A decision framework for the preservation of transparent papers.” Journal of the Institute of Conservation. 38, No. 1, 2015, 118–126. Online here
- Yates, Sally Ann. “The Conservation of 19th Century Tracing Paper.” The Paper Conservator 8, 1984, pp. 20–39, with short bibliography of publications containing useful information on tracing paper.
Cardboard/Artist's Board/Illustration Board
(See also General References)
- Futernick, Robert. “Methods and Makeshift: Hinging Artifacts to Matboard.” The Book and Paper Group Annual 3, Washington DC: AIC, 1984, pp. 68–70.
- Gould, Barbara. “The Removal of Secondary Supports from Works of Art on Paper.” The Book and Paper Group Annual 6, 1987.
- Keyes, K. M. “A Method of Conserving a Work of Art on a Deteriorated Thin Surface Laminate.” The Paper Conservator 10, 1986, pp. 10–17.
(See also General References)
- Cohn, Marjorie. Wash and Gouache: A Study of the Development of the Materials of Watercolor. Cambridge, MA: The Center for Conservation and Technical Studies, Fogg Art Museum, 1977.
- Walsh, Judith. “Observations on the Watercolor Techniques of Homer and Sargent.” American Traditions in Watercolor: The Worcester Art Museum Collection. Susan E. Stickler, ed. New York: Abbeville Press, 1987, pp. 44–65.
Artists' Printing Papers
(See also General References)
- Dyson, A. Pictures to Print: The 19th Century Engraving Trade. London: Farrand Press, 1984.
- Lalanne, Maxime. A Treatise on Etching. London: Sampson Law, Marston, Searle and Rivington, London, 1880.
- Lumsden, E.S. The Art of Etching. New York: Dover, 1924.
- Perknson, Roy. “Degas's Printing Papers.” Edgar Degas: The Painter as Printmaker. Sue Walsh Reed and Barbara Stern Shaprio. Boston: Little, Brown and Company, 1984, pp. 255–261.
- Robison, Andrew. Paper in Prints. Washington, DC: National Gallery of Art, 1977.
- White, C. Rembrandt as an Etcher London: Zwemmer, 1969.
(See also General References)
- Bosch, Gulhar and Guy Petherbridge. “The Materials, Techniques and Structures of Islamic Bookmaking.” Islamic Bindings and Bookmaking. Gulhar Bosch, John Carswell and Guy Petherbridge. Chicago: The Oriental Institute, 1981, pp. 23–84.
- Gaur, Albertine. Writing Materials of the East. London: The British Library, 1979.
- Losty, Jeremiah, P. The Art of the Book in India. London: The British Library, 1982.
- Snyder, J.G. “Appendix 10: Study of the Paper of Selected Paintings from the Verer Collection.” G.D. Lowry and M.C. Beach. An Annotated and Illustrated Checklist of the Verver Collection. Arthur M. Sackler Gallery, Smithsonian Institution, Washington. Seattle: University of Washington Press, 1988, pp. 425–440.
- Zhou, Bao Zhong. “The Preservation of Ancient Chinese Paper.” The Conservation of Far Eastern Art, Preprints of the Contributions to the Kyoto Congress, 19–23 September 1988. London: IIC, 1988, pp. 19–21.
(See also General References)
- Barrett, Timothy. Nagashizuki: The Japanese Craft of Hand Papermaking. North Hills, PA: Bird and Bull Press, 1979.
- Fletcher, Shelley and Judy Walsh. “The Treatment of Three Prints by Whistler on Fine Japanese Tissue.” Journal of the American Institute for Conservation 18, No. 2, 1979, pp. 118–127.
- Inaba, M. and R. Sugisita. “Permanence of Washi (Japanese Paper). The Conservation of Far Eastern Art: Preprints of Contributions to the Kyoto Congress. London: IIC, 1988.
- Keyes, Keiko. “Japanese Print Conservation - An Overview.” The Conservation of Far Eastern Art: Preprints of Contributions to the Kyoto Congress. London: IIC, 1988, pp. 30–36.
- Keyes, Keiko. “The Use of Friction Mounting as an Aid to Pressing Works on Paper.” AIC Book and Paper Group Annual 3, 1984, pp. 101–104.
- Nicholson, C. “The Conservation of Three Whistler Prints on Japanese Paper.” The Conservation of Far Eastern Art: Preprints of Contributions to the Kyoto Congress. London: IIC, 1988, pp. 39–43.
- Smith, C. “The Use of Paper Suction Table in Flattening and Drying Moisture-Reactive Japanese Tissues.” AIC Poster Paper Text, 1982.
(See also General References)
- Chandler, David. “Edgar Degas in the Collection of the Art Institute of Chicago: An Examination of Selected Pastels.” Degas: Form and Space. Paris, Centre Culturel du Marais, 1984, pp. 443–448.
- Gagnier, Richard and Anne Maheux. “The Mounting of Over-size Works on Paper at the National Gallery of Canada.” Handout Symposium 88, Ottawa, Canada, 1988, 6pp.
- Jenkins, Penny. “India Laid Prints Meeting.” Paper Conservation News, No. 49, March 1989.
- Jenkins, Penny. “Preparation of India Proof Prints.” Typescript of notes from an interview with Philip McQueen, Nov. 15, 1988, 3 pp.
- King, Antoinette. “Changes of the Collage ‘Roses’ by Juan Gris.” Conservation and Restoration of Pictorial Art. Norman Brommelle et al., eds. IIC London: Butterworths, 1978, pp. 234–238.
- McAusland, Jane and Phillip Stevens. “Techniques of Lining for the Support of Fragile Works of Art on Paper.” The Paper Conservator 4, 1979, pp. 33–44.
- Schulte, Elizabeth Kaiser, Margaret Holben Ellis, and Antoinette King. “An Approach to the Conservation Treatment of Paul Klee Drawings.” The Book and Paper Group Annual 5, 1986, pp. 19–32.
- Sugarman, Jane. “Observations on the Materials and Techniques Used in 19th Century American Architectural Presentation Drawings.” The Book and Paper Group Annual 4, 1986, pp. 39–60.
- Volent, Paula. “Contemporary Techniques of Mounting Paper to Canvas.” The Paper Conservator 10, 1986, pp. 18–23.
(See also General References)
- “Conservation of Wallpaper.” Special issue of the Journal of the American Institute of Conservation. Spring, 1981.
- Clise, D. & Draper, B. 2007. “Jean Zuber et Compagnie’s Le Paysage à Chasses at Willow Wall: Removal, Treatment, and Reinstallationof an Early Nineteenth-Century Scenic Wallpaper”. The Book and Paper Group Annual. Volume 26, pp. 9-20.
- Entwisle, E.A. A Literary History of Wallpaper. London: B.T. Batsford, 1960.
- Frangiamore, Catherine Lynn. Wallpapers in Historic Preservation. Washington, D.C.: National Park Service, U.S. Department of the Interior, 1977.
- Gilmore, A.M., 1981. “Wallpaper and Its Conservation: An Architectural Conservator's Perspective”, Journal of the American Institute for Conservation, Vol. 20, No. 2, Conservation of Historic Wallpaper, pp. 74-82.
- Greysmith, Brenda. Wallpaper. New York: MacMillan, 1976.
- Harroun, S.G., Bergman, J., Jablonski, E. and Brosseau, C.L., 2011. “Surface-Enhanced Raman Spectroscopy Analysis of House Paint and Wallpaper Samples from an 18th Century Historic Property”. Analyst, Volume 136. Pp. 3453-3460.
- Lynn, Catherine. Wallpaper in America from the 17th Century to World War I. New York: W.W. Norton, 1980.
- Mapes, P. 2015. Historic Wallpaper Conservation. [Accessed 7th April 2015].
- McClelland, Nancy V. Historic Wallpapers from Their Inception to the Introduction of Machinery. Philadelphia and London: J.B. Lippincott, 1924.
- McClintock, T.M., 2002. “Case Studies on the Effect of Conservation on the Appearance of Historic Wallpapers”. Restaurator. Vol.23, pp. 165-186.
- National Park Service. 2007. Wallpapers in Historic Preservation: History of Wallpaper Styles and their Use. Published: 26th April 2007. [Accessed 2nd April 2015].
- Nylander, Richard. Wallpapers for Historic Buildings. Washington, D.C.: The Preservation Press, 1983.
- Oman, Charles C. and Jean Hamilton. Wallpapers: An International History and Illustrated Survey from the Victoria and Albert Museum. New York: Abrams, 1982.
- Shelley, M. 1981. “The Conservation of the Van Rensselaer Wallpaper”. Journal of the American Institute of Conservation. Volume 20, Number 2, pp. 126-138.
- Teynac, Francoise, Pierre Nolot, and Jean-Denis Vivien. Wallpaper: A History. New York: Rizzoli International Publications, 1982.
- Vitale, T. & Messier, P. 2004. “Historic Wallpaper Digitally Remastered: Early Twentieth-Century Block-Printed English Wallpaper in the Yin Yu Tang House at the Peabody Essex Museum”, The Book and Paper Group Annual, Volume 23, pp. 109-113.
- V&A. 2015. Flock Wallpapers. [Accessed 1st April 2015].
- Welsh, F.S. 2004. “Investigation, Analysis, and Authentication of Historic Wallpaper Fragments”. Journal of the American Institute of Conservation. Vol. 43, No. 1, pp. 91-110.
(See also General References)
- Harding, E.G. “The ‘Inlaying’ of Works of Art on Paper.” Letter to the editor and response from Jane McAusland, Paper Conservation News No. 40, Dec. 1986, pp. 2–3.
(See also General References)
- Albright, Gary and T.K. McClintock. “The Treatment of Oversize Paper Objects.” Postprints of the AIC Book and Paper Group Meeting. Washington, DC: AIC, 1982, 6 pages.
- Eckmann, Inge-Lise. “The Lining of a Super-Sized Contemporary Drawing.” AIC Preprints. Washington, DC: AIC, 1985, pp. 36–43.
- Fairbrass, Sheila. “The Problems of Large Works of Art on Paper.” The Paper Conservator 10, 1986, pp. 3–9.
- Hamm, P. Dacus. “Treatment of an Oversized, Hand-Drawn Shaker Map.” Book and Paper Group Annual 7, 1988, pp. 17–22.
- Nicholson, C. and Susan Page. “Machine Made Oriental Papers in Western Paper Conservation.” Book and Paper Group Annual 7, 1988, pp. 44–51.
- Owen, Antoinette. “Treatment and Mounting of a Poster ‘Angleterre’ by A.M. Cassandre.” Journal of the American Institute for Conservation 24, No. 1, 1984, pp. 23–32.
- Potje, Karen. “A Travelling Exhibition of Oversized Drawings.” Book and Paper Group Annual 7, 1988, pp. 52–57.
- Volent, Paula. “Consideration in the Acquisition and Care of Oversized Contemporary Drawings.” Drawing 11, No. 2 (July/August) 1989, pp. 30–34.
Three-Dimensional Paper Objects
(See also General References)
- Evetts, Debora E. “Treatment of Folded Paper Artifacts.” The Book and Paper Group Annual 6, 1987, pp. 35–39.
- Florian Papp Gallery. Rolled, Scrolled, Crimpled, and Folded: The Lost Art of Filigree Paperwork. New York: Florian Papp Gallery, 1989.
- Newman, Jerri, Margaret Leveque, and Leslie Smith. “An Interspeciality Approach to the Conservation of Multi-Media Objects.” Preprints of Papers Presented at the 15th Annual Meeting of the AIC. Vancouver, 1987, pp. 84–98.
- Nichols, K., Elgar, J., Gausch, K. 2006. “Illuminating the Way: Conservation of Two Japanese Paper Lanterns” Journal American Institute of Conservation, Volume 46, pp. 123-136.
- Two nineteenth-century Katsushika Hokusai paintings in the form of paper folding-lanterns were conserved for the exhibition "The Allure of Edo" at the Museum of Fine Arts, Boston. The paintings had been dismantled from their original mounts, and in doing so they were severely damaged. The article describes the conservation treatment and the process of determining the original shape of each lantern. Polyethylene foam mounts were made and the paintings, which were relined, were adhered to them. The treatment was successful and the article exemplifies a unique and complex treatment that returned the paintings to their intended three-dimensional format.
- Tombs, Rebecca. “Three Dimensional Objects of Paper.” Unpublished paper Queen's University Art Conservation Program, Kingston, 1982.
Fans and Screens
(See also General References)
- Armstrong, Nancy. The Book of Fans. Surrey: The Colour Library International Ltd, 1978.
- Kakoauei, M., Kakouei Ezbarami, M., and Kumaran, S., 2014. “History, Technology, and Treatment of a Painted Silk Folding Screen Belonging to the Palace-Museum of Golestan in Iran”. Fibres & Textiles in Eastern Europe, Vol. 22, No. 2(104), pp. 69-75.
- This article is a case study illustrating the treatment of a historical Chinese folding screen from the Palace-Museum of Golestan in Iran. The main aim of this study was to develop the conservation treatment using paper conservation techniques as a basis. To restore the folding screen, a method often used in paper conservation was adopted. Self-adhesive heat reactivated Japanese tissue paper was attached to support the silk, in order to avoid stitching through the painted surface. Tengujo Japanese tissue, with Lascaux 498 HV diluted with water (10%) were selected for the repairs. Lascaux 498 HV has a pH of 8 – 9, great flexibility, is reversible and soluble in acetone, toluene and xylene but insoluble in water once dry. The self-adhesive tissue paper was reactivated at 50 °C with a heated spatula.
- Koyano, Masako. Japanese Scroll Paintings, a Handbook of Mounting Techniques. Washington, D.C: FAIC, 1979.
- Maxson, Holly. “Design and Construction of a Support for a Folding Fan.” The Book and Paper Group Annual 4, 1986, pp. 33–38.
- Nishio, Y. 2001. “Maintenance of Asian Paintings II: Minor Treatment of Scroll Paintings”, The Book and Paper Group Annual, Volume 20, pp. 15-26.
- A well explained article describing how to repair tear, areas of loss, creases and damaged chords on Asian scroll paintings. The article is aided with images, diagrams and step-by-step explanations on how to carry out treatments.
- Toishi, K. and H. Washizuka. Characteristics of Japanese Art That Condition Its Care. Japanese Association of Museums, 1987.
- Webber, Pauline. “The Conservation of Fans.” The Paper Conservator 8, 1984, pp. 40–58.
(See also General References)
- Moir, Gillian. “The Care of Papier-M&acaron;ché.” History News 35, No. 6, June 1980, pp. 57–58.
- van der Reyden, Dianne and Don Williams. “The Technology and Conservation Treatment of a 19th Century Paper-Mache Chair.” AIC Preprints. Chicago Meeting. Washington, DC: AIC, 1986, pp. 125–142.
(See also General References)
- Baynes-Cope, A.D. The Study and Conservation of Globes. Vienna: Internationale Coronelli-Gesellschaft, 1985.
- Lewis, Gillian, Anne Leane, and Sylvia Sumira. “Globe Conservation at the National Maritime Museum, London.” The Paper Conservator 12, 1988, pp. 3–12.
- Leyshon, Kim Elizabeth. “The Restoration of a Pair of Senex Globes.” The Paper Conservator 12, 1988, pp. 13–20.
- McClintock, T.K., 2002. “Observations On The Conservation Of Globes”, Studies in Conservation, Volume 47. Special Issue: Contributions to the Baltimore Congress, 2-6 September 2002. Works of Art on Paper Books, Documents and Photographs: Techniques and Conservation. Pp. 135-138.
- Globes are also often made from plaster, wood, metal, and have varnished and painted surfaces. A conservator of globes must also have conservation knowledge on these materials in order to make the treatment credible.The article gives reasons to why the conservation of globes falls under the role of the paper conservator rather than an objects or decorative arts conservator, even though the object is not solely made out of paper. McClintock writes that it is on the globe’s paper surface that the design and function of the globe is found, and it is the paper which is the most susceptible to damage. The author also explains the structure of a globe, describing the way the paper is prepared in order to paint and varnish it, without damaging the paper, as well as the wooden and metallic components that make up its structure.
- McClintock, T.K., Bigrigg, Lorraine & LaCamera, Deborah. 2015. “Case study: conservation and restoration of a pair of large diameter English globes”, Journal of the Institute of Conservation, 38:1, 77-91, DOI: 10.1080/19455224.2015.1007072
- The globes illustrated in these case studies were in very poor condition and hard to read. This article not only looks at the conservation treatment of the globes but also at the development of filling losses using digital photography and archival printing, which helped maintain the integrity of the globes as works of cartography. It was possible to use digital photography to recreate the losses because the same globe gores were printed in an Atlas, and could be used as models to reproduce the scans.
- Sumira, Sylvia. “Conservation Treatment of Globe Surfaces.” IIC Preprints, Brussels Congress: Cleaning, Retouching and Coatings. John S. Mills and Perry Smith, eds. IIC, 1990, pp. 56–58.
- Stevenson, E.L. Terrestrial and Celestial Globes: Volumes I and II. New Haven: Yale University Press, 1921.
- van Der Reyden, Dianne. “The Technology and Treatment of a Nineteenth Century American Time-Globe.” The Paper Conservator 12, 1988, pp. 21–30.
Traditional Non-Paper Supports
(See also General References)
- Bell, Lilian. Papyrus, Tape, Amatl, and Rice Paper; Paperrmaking in Africa, the Pacific, Latin America and Southeast Asia. 2nd edition. McMinnville, Oregon: Liliacea Press, 1985.
- Lenz, Hans. El Papel Indigena Mexicano, Historia y Supervivencia. English translation by H. Murray Cambell 1961. Mexico D.F.: Rafael Loeray Chaven, Editorial cultura, 1948. (amate)
- Shagun, Fray Bernardino de. Florentine Codex, General History of the Things of New Spain. Translated by Charles Dibble and Arthur, J.O. Anderson, in thirteen parts. Santa Fe: School of American Research and the Museum of Mexico, 1963. (amate)
(See also General References)
- Elliott, Frances and Eric Harding. “A Modern Approach to Papyrus Conservation: Materials and Techniques as Applied at the British Museum.” The Paper Conservator 11, 1987, pp. 63–68.
- Evans, Debra, D. Hamburg, and M. Mickelson. “A Papyrus Treatment: Bringing the Book of the Dead to Life.” Papers Presented at the Art Conservation Programs Training Conference. Newark, DE: University of Delaware, 1983, pp. 109–126.
- Grasselli, Jeanette. “Papyrus: The Paper of Ancient Egypt.” Analytical Chemistry. 55 1220A, 1983, 7 pp.
- Noack, Gisela. “Conservation of Yale's Papyrus Collection.” The Book and Paper Group Annual 4, 1986, pp. 61–73.
- Sturman, Shelly. “Investigations into the Manufacture and Identification of Papyrus.” Recent Advances in the Conservation and Analysis of Artifacts. London: University of London, Summer Schools Press, 1987, pp. 263–265. Includes extensive bibliography.
(See also General References)
- Lawson, Peter. “Conservation of Palm Leaf Books.” Conservation News 36, 1983, pp. 14–19.
- Van Dyke, Y. 2009. “Sacred Leaves: The Conservation and Exhibition of Early Buddhist Manuscripts on Palm Leaves”. The Book and Paper Annual, Vol. 28, pp. 83-97.
- The article describes the material composition and preparation of a collection of Indian paintings on palm leaf and paper, from the Metropolitan Museum of Art. The author describes in detail the different types of palm leaves and their physical properties as well as the methods used to process the leaves to make them suitable to paint on. These methods include: smoking, soaking, being boiled in water, hung over a charcoal fire and dried by the sun or kiln.
- The pigments were identified, though the method of identification was not mentioned, and due to the brittle nature of the palm leaf these pigments had to be consolidated. The choice of consolidant was made based on the desired working properties, which included strength, ageing, flexibility, viscosity, aesthetic and penetration. Gelatines and methyl cellulose were tested on the manuscript but they were not strong enough, left tidelines and dried glossy. Isinglass was chosen and used as a warm solution at 1%, this adhesive proved to be the best consolidant for both the flaking paint and the actual palm leaf. The leaves were humidified to rehydrate them and reduce the planar distortion, once humidified the leaves were less brittle so they could be more easily repaired using acrylic-dyed Japanese tengujo papers. The article also described the ethical consideration made when treating these objects, the storage solutions adopted to safely house the manuscript, and the exhibition conditions including mounting and display.
- The paper is a very detailed and comprehensive conservation case study, which included the historical context of the object, material analysis, ethical considerations and future storage recommendations. Though the paper was aimed at professionals in conservation, the article appeals to a wider audience, providing useful information to researchers, historians and curators; this added importance to the content as it promoted interdisciplinary collaboration and awareness.
(See also General References)
- Abt, Jeffrey and Margaret Fusco. “A Byzantine Scholar's Letter on the Preparation of Manuscript Vellum.” Journal of the American Institute for Conservation 28, No. 2., 1989, pp. 61–66.
- Cains, Anthony. “Repair Treatments for Vellum Manuscripts.” The Paper Conservator 7, 1982/83, pp. 15–23.
- Chahine, Claire. “Le Parchemin.” Proceedings of the International Symposium: Conservation in Archives, Ottawa, May 10–12, 1988 International Council on Archives, 1989, pp. 11–24.
- Clarkson, Christopher. “Preservation and Display of Single Parchment Leaves and Fragments.” Conservation of Library and Archive Materials and The Graphic Arts. Guy Petherbridge, ed. London: Butterworths, 1987.
- Forstmeyer, K., 2012. “Parchment Leafcasting Revisited”, Journal of the Institute of Conservation, 35:2, pp.219-229.
- The repair of a difficult area of loss on a piece of parchment can achieved by using a vacuum table and making a suspension of animal collagen fibres to create ‘reconstituted parchment’. The technique of wet-casting pulp dispersions on an object is discussed, as well as the application of reconstituted parchment with different adhesives, and methods of dyeing the fill to achieve the most appropriate colour.
- Munn, Jesse. “Treatment Techniques for the Vellum Covered Furniture of Carlo Bugatti” The Book and Paper Group Annual 8, Washington, DC: AIC, 1989, pp. 27–38.
- Reed, R. Ancient Skins, Parchments and Leathers. London: Seminar Press, 1972.
(See also General References)
- Lee, Mary Wood. “Conservation Treatment of Structural Damage to Pith Paintings.” Paper presented at the AIC 18th Annual Meeting, Richmond, Virginia, May 29-June 3, 1990.
- Perdue, Robert E., Jr. and Charles. J. Kraebel. “The Rice-Paper Plant - Tetrapanax Papyriferum (Hook) Koch.” Economic Botany 15, No. 2, April-June, 1961, 165–179.
- Rickman, Catherine. “Conservation of Chinese Export Works of Art on Paper: Watercolors and Wallpaper.” The Conservation of Far Eastern Art: Preprints of Contributions to the Kyoto Congress. London: IIC 1988, pp. 44–51.
(See also General References)
- Green, Sara Wolf. “Conservation of Tapa Cloth: Filling Voids.” The Paper Conservator 11, 1987, pp. 58–62.
- Green, Sara Wolf. “Conservation of Tapa Cloth from the Pacific.” Preprints of Papers Presented at the 14th Annual Meeting of the AIC. Chicago, IL: 1986, pp. 17–31, with earlier bibliography.
(See also General References)
- Douglas, Robyn. Architectural Drawings on Drafting Cloth. Unpublished report, Kingston: Queen's University Art Conservation Program, 1989.
- Lathrop, Alan. “The Provenance and Preservation of Architectural Records. The American Archivist 43, No. 3, Summer 1980, pp. 325–380.
Contemporary Non-Paper Drawing Supports
(See also General References)
- Hodges, E., ed. The Guild Handbook of Scientific Illustration. New York: Van Nostrand Reinhold, 1988.
- Williams, R. Scott. CCT Analytical Report, ARS Analytical Report No. 2631, Geofilm, CCI Registry File No. 7034 18–11, Ottawa, Canada: CCI, Sept. 25, 1987.
History of This Chapter
In 2009, the Foundation for Advancement in Conservation (FAIC) launched the AIC Wiki with funding assistance from the National Center for Preservation Technology and Training (NCPTT), a division of the National Parks Service. Along with catalogs from other specialty groups, the published Paper Conservation Catalog and the unpublished Book Conservation Catalog were transcribed into a Wiki environment. In 2017, Jennifer Evers reformatted this chapter by removing the legacy numbered outline format and improving internal links. In 2019, information from this page was moved to the [Paper Support] page.
Paper Conservation Catalog (print edition 1984-1994)
Prior to the creation of the AIC Conservation Wiki, this chapter was created in 1990 as Chapter 4: Support Problems of the 7th edition of the Paper Conservation Catalog, (print edition 1984-1994) by the following:
- Compilers: Thea Burns (Jirat-Wasiutynski) and Karen Potje.
- Contributors: Nancy E. Ash, Konstanze Bachmann, Cynthia Ball, Karl D. Buchberg, Robyn Douglas, Katherine G. Eirk, Theresa Fairbanks, Lynn Gilliland, Michele Hamill, Penny Jenkins, Anne Maheux, Jesse Munn, Yoshiyuki Nishio, Susan Page, Lois Olcott Price, Catherine Rickman, Christine Smith, Martha Smith, Rebecca Tombs, Elizabeth C. Wendelin.
- Editorial Board Liaison: Antoinette Dwan, Kimberly Schenck.
- Editorial Board: Sylvia R. Albro, Sarah Bertalan, Antoinette Dwan, Meredith Mickelson, Catherine I. Maynor, Kitty Nicholson, Kimberly Schenck, Ann Seibert, Dianne van der Reyden, Terry Boone Wallis.
|Paper Conservation Wiki|
|Examination and Documentation|
|Problems and Issues|
·Surface Cleaning ·Hinge, Tape, and Adhesive Removal ·Washing ·Sizing and Resizing ·Bleaching ·Alkalization and Neutralization ·Humidification ·Consolidation, Fixing, and Facing ·Backing Removal ·Mending ·Filling of Losses ·Drying and Flattening ·Lining ·Inpainting ·Matting and Framing ·Parchment ·East Asian Scrolls
|Book Conservation Wiki|
|Examination and Documentation|
|Structural Elements of the Book|
·Washing of Books
·Alkalinization of Books
·Leaf Attachment and Sewing Repair
·Use of Leather in Book Conservation
·Bookbinding Traditions by Region or Culture